Chapter 1 Introduction 1.1 Definition and Application of Hydrogel Hydrogel is a form of materials generally constructed by hydrophilic multiphase polymer mixture that may exhibit both solid-like and liquid-like properties. Its structural framework is formed from three-dimensional networks of randomly crosslinked polymeric chains that embody three different phases, namely solid polymer network matrix, interstitial water or biological fluid and ion species. A schematic drawing of the microscopic structure of charged hydrogel is shown in Fig. 1.1. The solid portion of the hydrogel is a network of crosslinked polymer chains where their three-dimensional structure is usually described as a mesh, with the interstitial space filled up with fluid. The meshes of networks hold the fluid in place and also impart rubber-like elastic force that can compete with the expansion or contraction of the hydrogel, thus providing the solidity of the hydrogel. The interstitial fluid phase mobile anion mobile cation fixed charge group undissociate ionizable group network chain crosslink Fig. 1.1 Schematic microscopic structure of charged hydrogel H. Li, Smart Hydrogel Modelling, DOI 10.1007/978-3-642-02368-2_1, C Springer-Verlag Berlin Heidelberg 2009 1 2 1 Introduction crosslinked polymer network may be formed physicochemically, for instance, by hydrogen bonding, van der Waals interaction between chains, covalent bond, crystalline, electrostatic interaction or physical entanglements. For the fluid phase of the hydrogel, it fills up the interstitial pores of the network and makes the hydrogel wet and soft, which is similar to biological tissues in some respects. Regarding the ionic phase of the hydrogel, generally it is composed of ionizable groups bound onto the polymer chains and a number of mobile ions which include counterions and co-ions due to the presence of electrolytic solvent that surrounds the hydrogel. The ionizable groups may dissociate in solution completely for strong electrolyte or partially for weak polyelectrolyte groups, and the network is left with the charged groups fixed to its chains. There is a considerable variety of materials in either naturally existing or synthesizing, as examples of swellable hydrated polymeric gels. Crosslinked guar gum and collagens are the examples of the natural polymer that are modified to produce hydrogels. Examples of the synthetic hydrogels include N-isopropylacrylamide (NIPA), poly(acrylic acid) (PAA), poly(acrylonitrile) (PAN), poly(acrylamide) (PAM), poly(acrylonitrile)/poly(pyrrole) (PAN/PPY), poly(vinyl alcohol) poly(acrylic acid) (PVA–PAA), poly(hydroxyethyl methacrylate) (PHEMA). Depending on the preparation history of the hydrogel and the physical and chemical characteristics of the polymer, hydrogels may be categorized further into subclasses. For example, hydrogels can be synthesized to be either neutral or ionic, determined by the chemical characteristics of the pendant groups fixed onto the polymer matrix. From the point of physical mechanism, if the overall structure of hydrogels is homogeneous, the polymer chains have a high degree of mobility. If it is heterogeneous, there is a great deal of internal polymeric interactions and the polymer chains are virtually immobile at the molecular level. However, the eventual stability of the hydrogel depends on the interaction between the polymer matrix network and the aqueous medium where the hydrogel is immersed. A smart or called environmental stimuli-responsive hydrogel is often synthesized when an ionic monomer is incorporated into the hydrogel network. The resulting charged group is generally termed the fixed charge since its mobility is much less than that of freely mobile ions within the interstitial fluid. The fixed charge groups produce electrostatic repulsion force among themselves, which influences greatly the expansion or contraction of hydrogel network. It is therefore known that the fixed charge density has an important effect on the electrostatic force and is able to play a substantial role in the change of degree of swelling/deswelling of the hydrogel. The smart hydrogel is increasingly attracting more and more attention due to its great promise for a wide range of bioengineering applications, especially in bio-micro-electro-mechanical systems (BioMEMS). This kind of hydrogels is able to demonstrate the unique property of undergoing discrete or continuous volume transformation or volume phase transition in response to infinitesimal changes in external environment conditions, such as solution pH, electric field, temperature, solvent composition, glucose/carbohydrates, salt concentration or ionic strength, light/photon, pressure, coupled magnetic and electric fields. Usually the 1.2 Historical Development of Modelling Hydrogel 3 Fig. 1.2 Reversible expansion or contraction of the smart hydrogel due to environmental changes volume transformation or volume phase transition due to environmental changes is reversible when the external environmental stimuli disappear (Fig. 1.2). These magnificent features make the hydrogel better known as smart (intelligent) or environmental stimuli-responsive hydrogels. Due to the wonderful properties of the smart hydrogels, such as reversible swelling/deswelling behaviour, sorption capacity, novel mechanical property, high ionic conductivity, high environmental sensitivity, permeability and surface property, the hydrogels provide platform for creating novel smart materials for a wide range of BioMEMS applications as the highly manoeuvrable smart and adaptive hydrogels are able to respond to environmental changes and eventually induce structural changes without requirement of external power source. Examples of the successful BioMEMS applications of the smart hydrogels include microfluidic control, biomimetic biosensor/ bioactuator, separation process and artificial muscle. Another exceptional promise of the hydrogels is their biocompatibility and biostability potentials, by which the hydrogels become excellent substitution for the human body tissues or biomimetic applications. There are also extensive explorations of the hydrogels in the medical and pharmaceutical applications, such as drug delivery system, articular cartilage, biomaterial scaffold, corneal replacement and tissue engineering. 1.2 Historical Development of Modelling Hydrogel As mentioned above, the smart hydrogels as three-dimensional crosslinked hydrophilic polymer networks are capable of swelling/deswelling reversibly in water and retaining large volume of liquid in swollen state. They may perform dramatic volume transition in response to a variety of physical and chemical stimuli, where the physical stimuli include temperature, electric or magnetic field, light, pressure and sound, while the chemical stimuli include pH, solvent composition, ionic strength and molecular species. Owing to their smart or stimulus-responsive property, the hydrogels have been used for applications in numerous areas such as mechano-chemical actuators and sensors, environmental remediation, microfluidic 4 1 Introduction control and separation, drug delivery and BioMEMS, artificial muscles and biomaterials for biomedical and tissue engineering. The characteristics of volume transition of the smart hydrogels have drawn considerable attentions. The literature search reveals that numerous studies have been done. However, the majority of them are experimental based. For the few published studies that conducted mathematical modelling and numerical simulation, results were far from satisfactory, where comparisons with experimental data show significant discrepancies. This has resulted in ad hoc studies of these hydrogel materials mainly conducted by trial and error. This is a very time-consuming and inefficient process, and certain aspects of fundamental knowledge can often be missed or overlooked, resulting in off-tangent research directions. Thus it is absolutely necessary to establish a theoretical platform through development of better mathematical models with excellent capability of characterizing the multiphase hydrogels in multiphysics environmental conditions, and also the powerful numerical simulations for solution of these challenging highly nonlinear coupled models, where multiphysics and multiphase are common requirements. In addition, with increment of biomedical applications, the smart hydrogels with more complex shapes are increasingly required and the accurate dimensional measurement of their volume transitions is becoming a challenge in experimental analysis. Therefore, computational modelling and simulation to predict the performance of the smart hydrogels become a critical tool for understanding of the characteristics of the smart hydrogels. On the other hand, when the optimization of hydrogel characteristics is required for specified applications, ready modelling and simulation will prove indispensable. In the past several years, some encouraging progresses were achieved in computational prediction of volume transition behaviours of the hydrogels in various case studies. In this section, we summarize and review several typical existing models that have been widely used, and then categorize them roughly into two groups, the steady-state models for equilibrium simulation and the transient models for kinetics simulation, respectively. Comments on the models and several key parameters are also given for full understanding. It should be pointed out here that the present category is not done exactly since some models can be employed for both equilibrium and kinetics simulations. However, all we do here is to provide readers a clear outline of historical development and technological application of mathematical models and numerical simulations of the smart hydrogels. We believe that the review on the achievements and challenges is greatly instrumental to further study in this aspect. 1.2.1 Steady-State Modelling for Equilibrium of Smart Hydrogels The present steady-state models focus on the responsive behaviours of the smart hydrogels at different equilibrium states. We provide an overview of the developed models in both macroscopic and molecular levels for simulation of volume 1.2 Historical Development of Modelling Hydrogel 5 transition behaviours of the smart hydrogels. The laws of energy, mass and momentum conservations provide good starting points for developing mathematical models for the hydrogel volume transition. Thermodynamic models, transport models, multiphase mixture theory and molecular simulation are discussed in details. Thermodynamic models provide the qualitative description of equilibrium volume transition of the hydrogels. Both the transport models and multiphase mixture theory are able to predict the equilibrium and kinetics volume transitions of the hydrogels. Molecular simulation provides the mechanism for understanding the hydrogel volume transition. Several key parameters are summarized for future model development. 188.8.131.52 Mathematical Models and Simulations The volume transition of the smart hydrogel involves intricate chemical process, hydrophilic, hydrophobic and electrostatic interactions and mechanical deformation. In order to accurately characterize the volume transition behaviour of the hydrogel, it is absolutely necessary to develop computational models incorporating the multidiscipline complexity. Conservation laws, including the energy conservation law, the mass conservation law and the momentum conservation law, are good starting points for developing mathematical models simulating the volume transitions of the smart hydrogel. Four types of the typical existing steady-state models are thus reviewed here. 1. Thermodynamic Models Energy balance arises from the energy conservation law, which may be characterized by thermodynamics theory. Thermodynamic models offer simple approaches in order to describe the volume transition behaviours of neutral or ionic hydrogels in equilibrium. The equilibrium state of volume transition of the smart hydrogel in solvent is reached when the solvent inside the hydrogels is in thermodynamic equilibrium with that outside. This can be characterized in terms of the free energy, the chemical potential or the related osmotic pressure. 2. Transport Models Mass conservation law can be transferred into a mathematical form of diffusion equations to describe the concentration distributions of mobile ions inside and outside the hydrogels, where the transport models account for osmotic pressure, electrical potential, hydrogel stress, and thus the hydrogel volume transition associated with diffusive flux of mobile ions. The models can provide both transient and equilibrium simulations for description of the volume transition behaviour of the ionizable hydrogels. 3. Multiphase Mixture Theory Momentum conservation law can describe the stress due to friction in a shear flow and in a compression or expansion flow. The multiphase mixture theory supposes that the volume transition of the elastic hydrogel is controlled by the friction force in the hydrogel network. It encompasses the flow-dependent 6 1 Introduction mechano-electro-chemical behaviours to balance the frictional force in hydrogels for description of volume transition behaviours of the hydrogel. 4. Molecular Simulation In order to deeply understand the volume transition behaviours of the hydrogel, an ideal approach is the modelling of various hydrophilic, hydrophobic and electrostatic interactions in molecular or even atomistic level, which is involved in the volume transition processes of the hydrogel. This can be achieved by molecular simulation, which incorporates various interactions with different energy expressions. Thermodynamic Models The most extensively used thermodynamic model was derived by Flory (1953) for description of the equilibrium volume transition of the hydrogels. The hydrogel at equilibrium state is treated as a special solution system, where the mesh chains cannot move freely to each other relatively, but the chains can become elongated in a non-interacting way during the volume transition process. The free energy of the neutral hydrogels is assumed to be a sum of the mixing free energy due to the mixing process and the elastic free energy due to the rubber elasticity. The osmotic pressure acting on the hydrogel network can be calculated according to the change of free energy. The osmotic pressure associated with the change of mixing free energy, π mix , is given by the Flory–Huggins polymer solution theory as follows (Flory 1953): πmix = − RT ln (1 − φ) + φ + χ φ 2 V1 (1.1) where R is the universal gas constant, T is the absolute temperature, V1 is the molar volume of solvent and χ is the polymer–solvent interaction parameter. ø is the polymer volume fraction of the hydrogel, thus (1−ø) is the solvent volume fraction. The osmotic pressure due to the change of elastic free energy, πel , is obtained by the rubber elasticity theory, which in turn is derived from the Gaussian chain model as follows: πel = − RT −1 1/3 2/3 Nc φ φ0 − φ/2 V1 (1.2) where ø0 is the polymer volume fraction at the relaxed state which may be taken as preparation state and Nc is average number of segments in the network chain. For highly crosslinked hydrogels, when the polymer chains contain fewer than 20 monomers between crosslinks, it is appropriate to use an expression for πel that assumes the non-Gaussian chain statistics (Peppas, 1986). Several expressions describing the volume transition of the non-Gaussian polymer networks were proposed by Kovac (1977) and Galli (1982). When the hydrogel volume transition reaches equilibrium, the total osmotic pressure of the hydrogel system, which is the sum of Eqs. (1.1) and (1.2), is equal to zero. 1.2 Historical Development of Modelling Hydrogel 7 According to the equations, the polymer volume fraction at equilibrium state øe can be calculated by the following equation: 2/3 ln (1 − φe ) + φe + χ φe2 + Nc−1 φe1/3 φ0 − φe /2 = 0 (1.3) To account for the steep or discrete volume transition of the hydrogel, the χ parameter is assumed to be concentration dependent in form of χ = χ1 + φχ2 (Erman and Flory, 1986). Both the parameters χ 1 and χ 2 are functions of temperature. Critical conditions for collapse of the neutral hydrogels require χ 1 = 1/2 and χ 2 = 1/3, which are easily met for a polymer–solvent system through adjustment of the crosslink density and/or attachment of charged ions onto the network chains. The attachment of charged ions brings about the translational entropy of the counterions, which gives rise to the change of free energy of ions. The osmotic pressure due to ions, π ion , is given as follows: πion = fRT/V r φ (1.4) where f is the charge density of the hydrogel, i.e. the fraction of segments bearing ionic groups. V r is the molar volume of the polymer monomer. Based on Eqs. (1.1), (1.2) and (1.4), the well-known Flory–Rehner relationship is obtained (Kovac, 1977): f 2/3 ln (1 − φ) + φ + χ φ 2 + Nc−1 φ 1/3 φ0 − φ/2 − V1 φ = 0 Vr (1.5) s in external solution results in variational disAdding salt with concentration Csalt tribution of mobile ions inside and outside the hydrogel. Influence of the electrolyte can be evaluated by the ideal Donnan equation, which gives rise to f 2/3 s −V1 φ = 0 (1.6) ln (1−φ)+φ+χ φ 2 +Nc−1 φ 1/3 φ0 − φ/2 −2(K−1)V1 Csalt Vr where K is the Donnan coefficient of the mobile ions inside and outside the hydrogel, and it is calculated by fφ K K+ −1=0 s V r Csalt When the concentration of external electrolyte is larger than that of counterions belonging to the polymer, and the concentration difference of the mobile ions between the external electrolyte and the internal hydrogel is comparable in 8 1 Introduction magnitude to the concentration, π ion of the hydrogel with ionizable groups in electrolyte solution can be expressed in term of ionic strength as follows: πion = RTV1 i2 c22 4I (1.7) where i is the degree of ionization, c2 is the concentration of ionizable polymer and I is the ionic strength of the medium for volume transition of the hydrogel. Based on Flory’s pioneering work, various modified models for predicting the volume transition behaviours of the hydrogel are proposed with the following assumptions: • The elastic, mixing and ionic contributions to the free energy are independent of each other • The chains possess the Gaussian statistics in approximation of the elastic contribution • The end-to-end distance of a chain scales linearly with the linear extension of the hydrogel, namely so-called affine assumption • The ionic contribution represents the coupled effect of the network being charged with the presence of mobile ions. The osmotic pressure originates from the electrostatically confined ions inside the hydrogel and the repulsive electrostatic interactions between the charged groups Based on Eqs. (1.1) and (1.7) as well as the phantom network model, Caykara et al. (2003) derived the following equation for predicting the equilibrium swelling behaviour of copolymeric hydrogels containing monoprotic acid moieties: Ka 10−pH + Ka 2 V1 fi2 − φ −2 ln (1 − φ) − φ −1 2 4IV r 2/3 1 − 2 V1 ρφ0 φ −5/3 =χ+ Mc (1.8) where M c is the average molecular weight between the crosslinks, Ka is the dissociation constant of the anionic polymer, fi is the molar fraction of the ionic unit in the hydrogel system, ρ is the density of the polymer network, pH is the pH value of medium surrounding the hydrogel and is the functionality at the crosslinking site. The equation can be used to predict the equilibrium volume transition behaviours of the copolymeric hydrogels containing diprotic and triprotic acid moieties and the amphiphilic hydrogels after proper modification of the expression for i in Eq. (1.7) (Sen et al., 1998, 2000; Caykara et al., 2000). The above equation is used to determine the M c and χ parameters of the copolymeric hydrogels. Additional contribution of electrostatic interaction to the free energy for ionizable hydrogels was taken into account by Fomenko et al. (2002). Kramarento et al. 1.2 Historical Development of Modelling Hydrogel 9 (2000) expressed the free energy of weakly charged hydrogel as a sum of six terms: (1) the elastic free energy, (2) the free energy of interaction of the monomer units, (3) the free energy gained from ion pairing, (4) the free energy associated with the translational entropy of mobile counterions inside the hydrogel and the outer solution, (5) the free energy of Coulombic interaction and (6) the free energy related to the combinatorial entropy of distribution of counterions between three possible states. The free energy was also described in terms of probability distribution function of different configurations (Huang et al. 2002). Hong and Bae (2002) combined the modified double-lattice model with Flory–Erman’s elastic model and the ideal Donnan theory to capture the swelling behaviours of the electrolyte-bounded hydrogels. A network parameter κ ranging from 0 to ∞ is employed to describe the constraints on fluctuations of junctions from the surrounding chains in which they are embedded (Erman and Flory, 1986; Hong and Bae, 2002). κ = 0 when the network approaches a “phantom network” in the limit of high volume transition, while κ→∞ if the network is an “affine network”. Contribution of hydrogen bonding to the free energy of hydrogels was also taken into account by several researchers. Annaka et al. (2000) incorporated a numerical constant Z to quantify the alteration of hydrogel osmotic pressure. The Z value depends on the chemical structure of hydrogen-bonded unit. The hydrogen bonding fraction was integrated into the mixing free energy term by Varghese et al. (2000). However, the separation of the free energy of hydrogels into independent terms, i.e. the additivity of the different free energy contributions, is questionable. These terms all depend on the configuration of mesh chains. Therefore, they should be connected by the nature of hydrogel structure. This assumes the random mixing of polymer and solvent in hydrogel system, but this cannot hold owing to the hydrogen bonding between water and hydrophilic polymer and possible hydrophobic hydration at small water content. It also regards polymer monomers as unconnected, and the conformational entropy of polymer chains and their interactions with the solvent molecules are separated. This underestimates the monomer correlation of polymer chains and hence overestimates the intra-chain monomer repulsion in good solvent. On the other hand, the Gaussian chain assumption, which is the basis of the elastic free energy for most thermodynamic models, overestimates the elastic free energy for stretched chains. This is attributed to the two effects. First, the chains in most hydrogels do not behave in a Gaussian way. Second, the chains are not long enough to be taken as Gaussian way since the number of monomers between two crosslinks, Nc , is often less than 100. In general, the parameters in the thermodynamic models are difficultly ascertained. Usually the estimated or best-fitted parameters are employed. This restricts the prediction accuracy of the thermodynamic models. Since they cannot incorporate temporal term into the system, the thermodynamic models cannot provide transient description for the kinetics volume transition behaviours of the hydrogel. This means that the thermodynamic models can be employed only for steady-state modelling of equilibrium of the smart hydrogels. The thermodynamic models provide a qualitative prediction of overall volume transition of the hydrogel. Acceptable agreement between the computational results and the experimental data may be 10 1 Introduction obtained if some parameters such as f and χ are taken as adjustable parameters. In applications of the thermodynamic models, the adjustment of these parameters is critical for simulation of volume transition behaviours of some hydrogels. Two of these parameters, the effective charge density and the polymer–solvent interaction parameter, are of most importance, and they are further discussed in detail as follows: 1. Effective Charge Density Polyelectrolyte hydrogels with counterions in solution are known to perform different degrees of counterion association with the polyelectrolyte. Ion pairing with subsequent aggregation of ion pairs into multiplet structure can lead to the appearance of a so-called super-collapsed state of hydrogels, where practically all counterions form ion pairs (Khokhlov and Kramarenko, 1994). This results in the reduction of the hydrogel charge density and the alteration of solution properties. Therefore, the volume transition of ionizable hydrogels is not always a monotonous increasing function with increasing ionic group contents (Durmaz and Okay, 2000; Melekaslan and Okay, 2000; Okay and Durmaz, 2002). The Flory–Rehner theory including the ideal Donnan equilibrium reveals that the existence of counterions inside the hydrogel is responsible for the observed volume transition behaviours. The fixed charge density calculated from the ionic group content cannot accurately describe the contribution of ionic groups to the free energy of the hydrogel. Kramarenko et al. (2000) proposed that three possible states of counterions could be distinguished, namely the free counterions in the solution and within the hydrogels and bound counterions forming ion pairs with the charged units of polymer chains. The fraction of bound counterions depends essentially on the dielectric constant of the medium inside the hydrogel, which changes during the hydrogel volume transition (Khokhlov and Yu, 1994). The effective charge density is used to take into account the reduction of the charge density of hydrogels. It is obvious that the effective charge density is dependent on the hydrogel composition. For example, the effective charge density feff of poly(acrylamide(AAm)-co-sodium acrylate) hydrogels swollen in aqueous NaCl solution is a function of sodium acrylate mole fraction fSA in form of feff = 1 − 19fSA + 155fSA2 (Okay and Sariisik, 2000). Simulation indicates that not all the fixed charges inside the hydrogel have influence on the hydrogel volume transition. The charge distribution of hydrogels also strongly affects the effective charge density and thus the volume transition behaviours. In the N-isopropylacrylamide (NIPAAm)/acrylic acid (AAc) hydrogels, the localized carboxyl ions are ineffective in preventing the thermally induced collapse at temperature above the volume phase transition temperature, compared with the randomly distributed carboxyl ions (Ogawa et al., 2002). The effective charge density of hydrogels changes with the alteration of volume transition medium. The effective charge density of the NIPAAm/2-acrylamido-2-methylpropane-sulfonic acid (AMPS) hydrogel in aqueous poly(ethylene glycol) (PEG)-300 solution was reported to vary with the volume fraction of PEG-300 øPEG in addition to the mole fraction of AMPS 1.2 Historical Development of Modelling Hydrogel 11 0.54 (1 − Aφ fAMPS according to feff = (31/Ns )fAMPS PEG ), where A is a constant describing the fraction of trapped counterions that form ion pairs in pure PEG and Ns is the number of segments on the network chains (Melekaslan and Okay, 2000). Electrokinetic studies also manifest that the effective charge density of poly(NIPAAm) varies with temperature (Makino et al., 2000a, b). The variation may be caused by the structural changes of the polymer chains and the water molecules in the hydrogels. However, there is still certain degree of ambiguity as to the state of the associated counterions, which result in the decrease of effective charge density. 2. Polymer–Solvent Interaction Parameter The polymer–solvent interaction parameter χ is a normalized interaction enthalpy. It is supposed that the nature of a pair interaction is not altered when the concentration of a component in the system changes. However, one must concede that the interaction of a given water molecule with another water molecule or with one of the polymer units in the hydrogel might be different. The interaction depends on the intensity of the molecule’s link to a polymer chain or on the degree to which the polymer unit is screened by surrounding water molecules. According to the regular solution theory, the Flory–Huggins interaction parameter χ is calculated from Hildebrand solubility parameters (Madkour, 2001) as follows: v (1.9) χ= (δ1 − δ2 )2 RT where v is the volume of a polymer segment, δ 1 and δ 2 are the Hildebrand solubility parameters of the polymer and the solvent, respectively. Three forces, namely the dispersion force, the polar force and the hydrogen bonding effect, make contribution to Hildebrand solubility parameter. However, their contributions are unequal (Hansen, 2000; Lindvig et al., 2002). Equation (1.9) clearly shows that the χ value decreases with the increase of temperature. This is observed in poly(methyl methacrylate (MMA))-methanol system, where χ = −1.985+919.23 T ±0.2 is obeyed with 95% confidence limit (Hassan and Durning, 1999). However, it is found that χ of protein-based hydrogels increases when temperature is below their phase transition temperature (Lee et al., 2001). It may be due to specific interaction, e.g. hydrophobic hydration, and free volume change with temperature. The ionization of dissociable groups in the hydrogels significantly changes the dispersion force, the polar force and the hydrogen bonding effect in the system, which has remarkable influence on the polymer–solvent interaction parameters. The polymer–solvent interaction parameter of AAc/methacrylated dextran hydrogels changes with varying ionization of AAc subject to different external pH conditions (Chiu et al., 2002), formulated by χ = 0.517 − 0.060fAAc − 3 2 − 0.310fAAc at pH 7.4, in which fAAc is the volume fraction of 0.061fAAc ionizable AAc in hydrogels (Chiu et al., 2002a, b). Hydrogel conformation and the hydrophobic hydration of the polymer chains may change during the volume transition process. Consequently, the 12 1 Introduction polymer–solvent interaction parameters of the hydrogels vary with the polymer concentration at different degrees of volume transitions. It was reported that χ ≈ 1/2 + φ/3 for poly(NIPAAm-co-AAc) hydrogel (Xue et al., 2001a, b). By considering the dependence of polymer–water interaction parameter on the polymer concentration as χ = 0.3875 + 0.518φ, the reentrant volume transitions of NIPAAm/AMPS hydrogels in aqueous PEG solution are successfully described (Melekaslan and Okay, 2001). Addition of organic solvent may change the structure of water surrounding the hydrophobic polymers and the hydrogen bonding network. This complicates the dependence of polymer–water interaction parameter with the polymer volume fraction. Chuang et al. (2000) used a ternary interaction parameter χT = −1.0 + 0.02φethanol + 1.3φ, depending on both polymer and ethanol concentrations, in which øethanol is the volume fraction of ethanol. The volume transition behaviour of poly(ethylene-co-vinyl alcohol) is reasonably predicted in the presence of this ternary interaction parameter. Dependence of polymer–water interaction parameter on both temperature and polymer concentration is also proposed for poly(N-t-butylacrylamide (TBA)co-AAm) hydrogels (Ozturk and Okay, 2002). Incorporating this sensitive dependence, the thermodynamic model may predict the volume transition of the hydrogels in satisfactory agreement to experimental data. Transport Models It is understood for the transport models that diffusion is a driving source to make the volume transition of the ionic smart hydrogels. Ion diffusive flux controls the osmotic pressure, the electrical potential of the network, the hydrogel stress, and thus the volume transition of hydrogel. Osmotic pressure is the directly driving force for volume transition of the smart hydrogels. Two expressions of the osmotic pressure lead to two different transport models. A transport model for prediction of the volume transition of the ionic smart hydrogels was employed by Wallmersperger et al. (2001), which couples the Nernst–Planck equations with the Poisson equation and the mechanical equilibrium equation to simulate the diffusive ionic concentration, the electric potential and the hydrogel volume transition. The Nernst–Planck equation is given as follows: Dk ∂ 2 ck ∂ck ∂ψ ∂ 2ψ + μ + μ z z c =0 k k k k k ∂x ∂x ∂x2 ∂x2 (1.10) where Dk , μk , ck and zk are the effective diffusivity, the mobility, the concentration and the valence of the kth ionic species inside the hydrogel, respectively. The index k (1, 2, 3, . . ., N) describes the N ionic species in the solution. ψ is the electric potential and it is modelled by the Poisson equation as F ∂ 2ψ =− εε0 ∂x2 N zk ck + zf cf k=1 (1.11) 1.2 Historical Development of Modelling Hydrogel 13 where ε0 is the dielectric constant of vacuum, ε is the relative dielectric constant of the solvent, F is the Faraday constant, cf and zf are the concentration and the valence of the fixed charge in the hydrogel, respectively. And the fixed charge concentration cf is related to the hydrogel volume transition by (Grimshaw et al., 1990) cf = 0 1 cf K H (K + cH ) (1.12) where H is the local hydration state of the smart hydrogel, K is the dissociation constant of the fixed charge group, c0f is the concentration of ionizable groups in the hydrogel before volume transition and cH is the concentration of hydrogen ions within the hydrogel. The mechanical equation governs the equilibrium of the hydrogel with the osmotic pressure, which is given as ∇ ·σ =0 (1.13) where σ is the stress tensor. The osmotic pressure π is calculated by the concentration difference of mobile ions between inside and outside the hydrogels, which is controlled by the diffusion process N π = RT chk − cks (1.14) k=1 where superscripts h and s represent the hydrogel and bulk solution, respectively. The first transport model thus consists of Eqs. (1.10), (1.11), (1.12), (1.13) and (1.14) which are nonlinearly coupled. A self-consistent solution is thus required by iteratively solving the Nernst–Planck equation, the Poisson equation and the mechanical equilibrium equation. This model simplifies the interactions in the hydrogel system. The required parameters in the formulation are easily determined. It is a convenient way for simulation of both equilibrium and kinetics of volume transition behaviours of ionic smart hydrogels in aqueous solutions. However, the model neglects the interactions between the polymer and water in the hydrogels, which include the hydrophilic and hydrophobic interactions and the hydrogen bonding effects. These forces may not be negligible in certain ionic hydrogels, compared with the osmotic pressure due to the concentration difference of ionic species. Their contributions should be incorporated for accurate prediction of the volume transition behaviours of the smart hydrogels. The second transport model considers the contributions of mixing, elastic and electrostatic free energies to the osmotic pressure, which was developed by Achilleos et al. (2000, 2001) for predicting the volume transition of polyelectrolyte hydrogels. The negligible inertia, electroneutrality and constant equal partial species densities are assumed in this model. The conservation laws for species mass and polymer mass, the mechanical balance and the overall charge balance for a mixture 14 1 Introduction of four components (k≡ 1–4, 1≡H2 O, 2≡Na+ , 3≡Cl− , 4≡p the polymer) are given as follows: dp wk wk dp wp wk −ρ + ∇ · jk − jp = 0 ρ (1.15) dt wp dt wp 1 dp wp 1 dp ρ + =0 (1.16) ∇ · vp + ρ dt wp dt ∇ · σ − ∇P = 0 p zk wk k=1 (1.17) M1 =0 Mk (1.18) where ρ, vP and P are the mixture density, the polymer velocity and the hydrostatic pressure, respectively. wk , jk and Mk are the weight fraction, diffusive flux and molecular weight of the kth species, respectively. dP /dt is the substantial derivative following the polymer velocity. The diffusive flux of the kth component is given as Mk ∇ · σ + zk ∇ψ jk = −Dk wk ∇πk + M1 (1.19) where π κ is the osmotic pressure of the kth component and it is derived from the free energy, which sums up the mixing, elastic and electrostatic contributions by p−1 p−1 χβp wβ Mk wβ Mk − Mβ Mβ β=1 β=1 2 z M1 Mk + CDH I 1.5 − 3zk I 1.5 + Cmf i2 wp − k +1 M1 IMk πk = ( ln wk + χkp wp + 1) − wP (1.20) where CDH and Cmf are two determined constants. The network stress is related to the polymer velocity vP and dP /dt and given as σ = φp dP σ − σ · ∇vP − ∇vTP · σ + σ ∇ · vP = G0 0 ∇vP + ∇vTP dt φp (1.21) where G0 is the hydrogel modulus, øp and φp0 are the polymer weight fraction in swelling and at gelation, respectively. The second transport model thus consists of Eqs. (1.15), (1.16), (1.17), (1.18), (1.19), (1.20) and (1.21) for simulation of both equilibrium and kinetics of volume transition behaviours of the polyelectrolyte hydrogels. This model may be understood as a transport model combined with the modified thermodynamic model. The volume transition of the hydrogels is still considered to be driven by the ionic diffusion, but the osmotic pressure is contributed by the mixing, elastic and electrostatic free energies. Though it takes into account the interactions between the polymer 1.2 Historical Development of Modelling Hydrogel 15 and solution in the hydrogels, it needs additional parameters to be determined. In general, it is accurate enough for the polyelectrolyte hydrogels with low degree of ionization. The transport model creates the relationship between the hydrogel volume transition behaviours and the ion diffusion process. It can thus provide both the equilibrium and kinetics descriptions of the volume transition behaviours of hydrogels, which is an advantage over the thermodynamic models. The model is able to achieve quantitatively the simulation of volume transition behaviours of the hydrogels when a suitable expression of osmotic pressure is employed. As well known, the parameters required by the transport models include mainly the diffusive coefficients of the mobile species and the elastic material properties of the hydrogels. Constant or concentration-dependent diffusive coefficients are employed. The elastic material properties of the polymer network may become difficult to be determined when the geometrical sizes of hydrogels are very small. Accurate values of the elastic material properties are important when the transport models are used. However, the elastic material properties are observed to change during the volume transition process. Therefore, it is necessary to make a further discussion of the relationship between the elastic material properties and the volume transition behaviours of hydrogels. The elastic property of hydrogels falls between two idealized limits, namely the affine and phantom. They relate the network structure to the elastic deformation subject to applied stress. In the affine model, crosslinks are assumed to be affine with respect to macroscopic strain and the fluctuations of the junctions are completely suppressed. In the phantom model, chains are considered immaterial or phantom and can freely cross each other. The chains exert forces on the crosslinks, which can move independently from the applied stress. The crosslink density has a primary effect on the elastic property of hydrogels. The crosslinking process of the polymer network matrix partially replaces the weak van der Waals intermolecular bonds by the strong covalent bonds, which evidently increases the mechanical strength of the polymeric network. The increase of crosslinking temperature is observed to monotonically decrease the elastic modulus due to the spatial heterogeneity of the crosslinked hydroxypropylcellulose (HPC) hydrogel (Valente et al., 2002). Theoretically, the increase of charge density should monotonically decrease the elastic modulus of hydrogels. However, the elastic modulus of the AAm/AMPS hydrogels is found to increase first with increasing the charge density and decrease subsequently (Okay and Durmaz, 2002). This demonstrates two opposite effects of charged groups on the elastic modulus of hydrogels: (1) the formation of multiplets to increase the elastic modulus of the ionic hydrogels and (2) the effect of electrostatic interaction of charged groups to decrease the elastic modulus. The initial increase of the modulus with increasing the charge density is connected with the condensation of counterions to ion pairs. The multiplets act as additionally physical crosslinks in the hydrogel and contribute to the elastic modulus by increasing the effective crosslink density of the hydrogel. The decrease of the elastic modulus at higher ionic group content is associated with the contribution of electrostatic interaction to the conformational change of the hydrogel chains. 16 1 Introduction The medium surrounding the hydrogels has remarkably influences on the elastic property of the hydrogels. Young’s modulus of pH-sensitive hydrogel is dependent on the medium pH (Johnson et al., 2002), while the negative dependence of the elastic modulus to temperature is observed in the crosslinked PAAm hydrogel (Muniz and Geuskens, 2001). In the collapsed state, the elasticity of poly(NIPAAm) hydrogel depends on the concentration and composition of salt in the aqueous solutions (Ikehat and Ushiki, 2002), probably due to the viscoelasticity from the shrinkage of the polymeric hydrogel. The elastic behaviour of hydrogels varies with the state of volume transition of the hydrogel. Young’s moduli of the hydrogels at swelling and deswelling states are remarkably different (Johnson et al., 2002). The modulus is inversely proportional to the swelling degree (Whiting et al., 2001). The relation between the shear modulus and the swelling degree for covalently crosslinked poly(aldehyde guluronate) hydrogels shows a linear logarithm relation (Lee et al., 2000). Three different regions of variation of Young’s modulus were reported with the degree of volume transition of a chitosan–poly(ethylene oxide) (PEO) hydrogel (Khalid et al., 2002). The first region is a slight decrease of Young’s modulus, which may be explained by the peripheral swelling of the hydrogel due to the uniform diffusion of the aqueous medium towards the centre of the hydrogel. The second region is a distinct decrease of Young’s modulus, which is ascribed to the arrival of the swelling border in the centre part of the hydrogel. Finally, a steady Young modulus of the polymeric network is described with a stationary hydration of the hydrogel. The relations between the solution fraction and the equilibrium shear modulus are derived with a statistical theory (Franse and Nijenhuis, 2000). Multiphase Mixture Theory In the multiphase mixture theory, it is assumed that the volume transition of the hydrogels is driven by the gradient of chemical or electrochemical potentials, which is balanced by the frictional force between the phases when one phase flows through the other (Zhou et al., 2002). The hydrogel system is divided into three phases, which are solid phase (denoted by s), water phase (denoted by w) and ion phase containing both anion (denoted by −) and cation (denoted by +). It is also assumed that the three phases are intrinsically incompressible, whereas the hydrogel as a whole is compressible through exudation of water. If both the body and the inertial forces are neglected, the momentum balance equations are given as ∇ ·σ =0 (1.22) − ρ w ∇μw + fws (vs − vw ) + fw+ (v+ − vw ) + fw− (v− − vw ) = 0 (1.23) − ρ + ∇ μ̃+ + f+s (vs − v+ ) + f+w (vw − v+ ) + f+− (v− − v+ ) = 0 (1.24) − ρ − ∇ μ̃− + f−s (vs − v− ) + f−w (vw − v− ) + f−+ (v+ − v− ) = 0 (1.25) 1.2 Historical Development of Modelling Hydrogel 17 where μ̃k is the electrochemical potentials for the kth species, μw is the chemical potential of fluid phase, fαβ is the frictional coefficient per unit tissue volume between the inter-diffusing α and β components and it is assumed to be symmetric, i.e. fαβ = fβα . The saturation condition is given as φj = 1 (1.26) j=s,w,+,− where j = s, w, + and −. φ j = dV j /dV is the volume fraction of the jth component. The continuity equation, electroneutrality condition and continuity equation of fixed charge group are given as follows: ∂ρ j + ∇ · (ρ j v j ) = 0 ( j = w,s, + , − ) ∂t (1.27) where v j is the velocity of component j and ρ j its mass density zj cj + zf cf = 0 j=+,− ∂(φ w cf ) ∂t + ∇ · (φ w cf vs ) = 0 (1.28) (1.29) For an isotropic hydrated charged hydrogel with infinitesimal deformation, the constitutive equations are given as follows: σ = −PI + λs tr(E)I + 2μs E 1 [P − RTξ (c+ + c− )] ρTw RT z+ Fψ μ̃+ = μ+ 0 + M ln (γ+ c+ ) + M + + Fψ RT z − μ̃− = μ− 0 + M ln (γ− c− ) + M − − μw = μw 0 + (1.30) (1.31) (1.32) (1.33) where I and E are the identity tensor and the elastic strain tensor of the solid phase, respectively; λs and μs are the Lamé coefficient and the shear modulus of solid phase, respectively; μk0 is the chemical potential at reference; ρTw is the true mass density of water; γ + and γ − are the activity coefficients of cation and anion, respectively; M+ and M− are the molecular weights of the cation and anion, respectively and ξ is the osmotic coefficient. The multiphase mixture model is applicable to the hydrogels with linear volume transition. It simplifies the interactions between the phases of the water, mobile ion and the polymer network, without consideration of variation of the hydrogel elastic properties in volume transition process. At the same time, the model assumes 18 1 Introduction the constant frictional coefficients between the phases. This directly restricts the applicability of the model. However, this model can describe both the equilibrium and kinetics of volume transition behaviours of the hydrogels. Molecular Simulation Unfortunately, the three kinds of the models discussed above, the thermodynamic models, the transport models and the multiphase mixture models, cannot evaluate the hydrophilic, hydrophobic and hydrogen bonding interactions involved in the hydrogels. However, the dynamic and structural characteristics of the hydrogels are accessible via molecular simulations. Over the past years, it is demonstrated that the molecular simulation is a uniquely useful tool for investigating the properties of polymer networks since it allows the construction and investigation of near-perfect model networks with well-characterized structures. It is able to examine the interaction between the electrolyte and the polymer matrix, which is much less understood. Fermi resonance perturbed Raman spectroscopy reveals that there exists weak polymer–electrolyte interaction between the poly(MMA) and the solvent molecules, ethylene and propylene carbonate (Ostrovskii et al., 2003). Ab initio molecular orbital calculation confirms that the hydrogen bonding hydration of the ion–water clusters to the polymers is destabilized by anions but stabilized by cations via ionic hydration in most cases (Muta et al., 2001a, b). It is understood that the volume transition of the hydrogels is based on the electron pair acceptance and electron pair donation change of water through the ionic hydration. Molecular simulation can provide examination of the mechanism of the volume transition. Using the Monte Carlo and molecular dynamics techniques, the swelling of weakly charged polyelectrolyte hydrogel in poor solvent is simulated (Lyulin et al., 1999). Splitting of the spherical polyelectrolyte globule into a dumbbell-type structure accompanied by a sharp increase in interaction occurs in the chain’s radius of gyration upon increasing in the Coulombic repulsion. By simultaneously treating the electrostatics and chain connectivity, the swelling of the crosslinked polyelectrolyte hydrogels is simulated by Monte Carlo technique (Schroder and Oppermann, 2002). This reveals that the assumption of Gaussian statistics in the hydrogel theories holds for the polymeric hydrogels but not for the polyelectrolyte hydrogels, whereas the affine assumption seems to be reasonable only for the polyelectrolyte hydrogels in equilibrium with pure solvent. Molecular dynamics simulation at an atomistically detailed level is carried out to predict the polymer volume transition by a two-step method in combination of the thermodynamic integration approach with Widom’s particle insertion method (Nick and Suter, 2001). The quality of simulation depends only on the energy model used, i.e. on the force field for the atom−atom interactions. The simulation indicates the concentration dependence of the polymer–water interaction parameter, expressed by χBPA−PC = 4.7 − 6.6φw for the bisphenol-A-polycarbonate (BPA-PC) and χPVA = 2.6 − 5.9φw for the poly(vinyl alcohol) (PVA), respectively, where øw is the volume fraction of water in the network. A statistical mechanics combined with the molecular dynamics simulation evaluates the influence of the volume transition on the entropy of mixing 1.2 Historical Development of Modelling Hydrogel 19 (Hansen, 2000). The loss in entropy due to the deformation of the chains takes on a negative value, and the final value of the mixing entropy decreases in both coiling and swelling. Molecular dynamics is also combined with other approaches to simulate the volume transition behaviours of the hydrogels. The swelling of athermal networks in an athermal hard sphere solvent is simulated by a discontinuous molecular dynamics combined with Monte Carlo simulation technique (Kenkare et al., 2000). An elastohydrodynamic approach is employed to model the hydrogel undergoing a large volume change during solvent diffusion (Barriere and Leibler, 2003). It couples the diffusion process with the large elastic deformation undergone by the polymer network. The solvent–polymer friction is described as a liquid flowing through a porous medium. The network elasticity over the range of volume fraction is divided into the isotropic and non-isotropic parts. Employing a Gibbs ensemble molecular dynamics method, the dynamic and structural results for equilibrium swelling of a model network in contact with different chain-like solvents are simulated by Lennard–Jones non-bonded interaction (Aydt and Hentschke, 2000). The swelling behaviour of model polymer networks in different solvents subject to the controlled thermodynamic conditions is simulated by a “two-box particle-transfer” molecular dynamic simulation method (Lu and Hentschke, 2002a, b). The solvent chemical potentials are calculated via the Widom’s test particle method for one-site solvents or the Rosenbluth sampling method for chain-like solvents, in which the simulation results are in qualitative agreement. Although the molecular simulation techniques provide the better understanding of the mechanism of both polymer–solvent interaction and polymer network conformation, the simulation is computationally intensive and time consuming. The selection of energy description models is also crucial to the simulation accuracy. It is limited to the hydrogels with relatively small structures. Therefore, it is difficult to practically predict the volume transition behaviour of the smart hydrogels with complex structures. Remarks We have discussed four types of models that are developed and based on different assumptions and approximations. With basic assumptions of the different contributions into the osmotic pressure, the thermodynamic models provide a tool for qualitative estimation of overall volume transition of the hydrogels in different equilibrium states. These thermodynamic models establish the relationship between the volume transition and the important material properties for the hydrogels. Transport models and multiphase mixture theory can quantitatively achieve both the equilibrium and kinetics simulations of volume transition behaviours of ionic smart hydrogels with complex shapes. The transport models suppose that the volume transition of the ionic smart hydrogels is driven by ionic diffusion and the osmotic pressure is the directly driven force for the volume transition of the hydrogel. These transport models establish the relationship between the volume transition behaviours of the hydrogels and the ion diffusion process and elastic stress. By formulation of 20 1 Introduction the osmotic pressure in the thermodynamic models, the transport models can also take into account important material parameters of the hydrogels. The multiphase mixture theory assumes that the hydrogels are composed of intrinsically incompressible solid phase, incompressible water phase and ion phase, and the volume transition of the hydrogels results from exudation of water driven by the gradients of chemical potential and electric potential. The theory generates the relationship between water flow and frictional forces. By integrating various hydrophobic, hydrophilic and electrostatic interactions involved, the molecular simulation makes it instrumental in investigate the mechanisms of volume transition of the hydrogels and to evaluate the influences of various environmental and material parameters. However, the requirement of intensive computation restricts its application to the small scale of the hydrogels. 184.108.40.206 Key Parameters in Steady-State Modelling for Equilibrium of Hydrogels It is known that there is a variety of parameters having influences on the volume transition behaviours of the smart hydrogels. For example, the ionic additives affect electrostatic interactions, the surfactants implicate the hydrophilic and hydrophobic forces and the organic solvents uphold the involvement of hydrogen bonding. Even the same additives may have remarkably different influences in different hydrogels. Successful mathematical models should be able to capture the influences of various parameters that significantly affect the volume transition of the smart hydrogel, which is definitely a challenge for modelling development and simulation. Several key parameters are summarized below. Hydrogel Composition The swelling/deswelling behaviour of the smart hydrogel is distinctly influenced by the monomer composition. Incorporating more hydrophilic or hydrophobic monomers in hydrogel composition is a useful approach to regulate the volume transition behaviour of the hydrogel. For example, the copolymerization of charged monomers is a well-tested strategy to increase hydrophilicity in polymeric chains and thus obtain the polyelectrolyte hydrogels. Among the charged monomers, AMPS and [(methacrylamido)-propyl]trimethyl ammonium chloride (MAPTAC) have received more attention due to their strongly ionizable sulfonate groups and complete dissociation in the overall pH range. It is demonstrated that the hydrogels incorporated with AMPS and MAPTAC can exhibit pH-independent swelling behaviour (Varghese et al., 2000; Ozmen and Okay, 2003). In general, the increase of charged monomer contents of the hydrogels increases the degree of volume transition (Katime and Rodriguez, 2001). One of the reasons is the simultaneous increase of counterions inside the hydrogels, which generates an additional osmotic pressure that expands the hydrogels. However, the degree of volume transition of the hydrogel is not always a monotonically increasing function of the charged monomer contents of the hydrogel. It may increase first with increasing ionic group concentration but then level off after passing a critical 1.2 Historical Development of Modelling Hydrogel 21 concentration due to the finite extensibility of the network chains and due to the ion pair formation (Durmaz and Okay, 2000; Melekaslan and Okay, 2000; Okay and Durmaz, 2002). Some hydrogels show a maximum degree of volume transition at certain ionic group concentrations. For example, the swelling ratio of poly(NIPAAm-co-AAc) hydrogel reaches to the largest value at 20 mol% of AAc content (Yoo et al., 2000), the poly(NIPAAm-co-methacrylic acid (MAAc)) hydrogel shows the largest swelling at 30 mol% of MAAc content (Diez-Pena et al., 2002) and the swelling ratio of poly(AAm-co-AAc) hydrogel reaches to the maximum value at 50 mol% AAc (Bouillot and Vincent, 2000). In exception, a slightly decreased swelling ratio with increasing content of charged monomer is observed in poly(NIPAAm)/chitosan hydrogels (Lee and Chen, 2001). It is proposed that addition of chitosan increases the hydrogel crosslinking and makes the network structure denser and more hydrophobic. When the zwitterionic monomer is appropriately introduced, the volume transition of the hydrogels may also be enhanced. The swelling ratio of thermo-sensitive poly(NIPAAm-co-1-vinyl-3-(3-sulfopropyl) imidazolium betaine (VSIB)) hydrogels in salt solution increases with increasing zwitterionic VSIB content (Lee and Yeh, 2000). Incorporating more hydrophilic neutral monomers may also increase the degree of the volume transition of corresponding hydrogels. The hydrophilic PEG and PEO polymers are often incorporated in the hydrogels to remarkably increase the volume transition (Cho et al., 2000; Bajpai and Shrivastava, 2002). The increase of the hydrophilic AAm content in the NIPAAm/AAm hydrogels gives rise to a higher equilibrium swelling ratio (Yildiz et al., 2002). The swelling ratio of the PVA/poly(NIPAAm) interpenetrating network (IPN) hydrogels increases with the increase of the hydrophilic poly(NIPAAm) content in the IPNs (Kim et al., 2003). However, the swelling ratio of the poly(2-hydroxyethyl methacrylate)(HEMA)/PEG IPN hydrogels increases first with increasing PEG concentration, but then decreases monotonously after PEG concentration increases beyond 0.33 g (Bajpai and Shrivastava, 2002). In general, the volume transition of the hydrogels decreases with integrating more hydrophobic comonomers (Bajpai and Giri, 2002). The swelling ratio of the poly(NIPPAm-co-AAm-co-HEMA) hydrogels decreases with increasing the content of hydrophobic AAm or HEMA (Yildiz et al., 2002). The formation of intermolecular hydrogen bonding between hydroxyl and amino groups decreases the hydrophilic group content of the hydrogels and thus the affinity towards water decreases. A more interesting observation is that, with increase of the hydrophobic monomer content of the di-n-propylacrylamide (DPAM), di-n-octylacrylamide (DOAM) and didodecylacrylamide (DDAM), the swelling ratio increases in the poly(NIPAAm) hydrogels (Xue and Hamley, 2002). The hydrogels even with the same composition may display different volume transition behaviours with different polymer architectures. The hydrogels made of random copolymer chains swell much larger than those composed of the triblock copolymer chains (Simmons et al., 2000; Triftaridou et al., 2002), which is attributed to the absence of microphase separation in the former type of network and the presence in the latter. 22 1 Introduction Preparation History Variation of the synthesis methods or formation conditions of the smart hydrogels provide another approach to control the volume transition of the hydrogel. The hydrogel microstructure and degree of topological constraint depend on the preparation conditions. The hydrophobic interactions in the temperature stimulus-responsive hydrogels also change with formation conditions (Suetoh and Shibayama, 2000). The monomer concentration has the most important effect, relatively compared with other preparation conditions. The swelling ratio can be controlled by preparing certain monomer concentration (Furukawa, 2000). The mechanism of volume transition of the poly(AAc) hydrogel is dependent on the preparing concentration of AAc in solution during γ-irradiation in addition to pH of the medium of the volume transition (Jabbari and Nozari, 2000). Solvent in the hydrogel preparation can change the porosity and crosslinking of the formed product. Ethanol as solvent is more effective than water for creating the porous structure of the hydrogels (Pradas et al., 2001). The primary cyclization in the hydrogels is facilitated by increasing the solvent concentration. The primary cyclization decreases the crosslinking density and increases the molecular weight between crosslinks. Consequently, this increases the degree of the volume transition of the hydrogels. On the other hand, the hydrogels prepared in bulk conditions exhibit much poorer volume transition behaviour than those in solution (Loh et al., 2001). Variation of physical preparing conditions, such as the heating time, radiation dose and applied electric field, also changes the volume transition of the hydrogel. The degree of the volume transition of poly(AAm-sodium acrylate-PVA) hydrogel increases to 1200 g water per 1 g swollen polymeric network after heat treatment at 120◦ C (Vashuk et al., 2001). The increasing porosity of the polymeric network results in the decrease of elastic modulus and thus the increase of the volume transition. Schmidt et al. (2003) reported that the poly(vinyl methyl ether) (PVME) structures formed by radiation crosslinking of PVME in aqueous solution can be microgel particles, porous hydrogels, branched molecules and homogeneous hydrogels, which are influenced by preparation parameters including radiation dose and irradiation temperature. The poly(NIPAAm-co-AAc) hydrogels prepared under constant electric current show gradual phase transition in response to temperature, which is in contrary to the general overall phase transition in aqueous solution (Shin et al., 2003). The copolymeric hydrogels start the phase transition from the section polymerized on the anode side and gradually change to the section polymerized on the cathode side when the temperature is increased. The gradual phase transition arises from the protonation of AAc near the anode and the ionization of AAc near the cathode by the electric current. The conditions of hydrogel pretreatment after preparation also have influences on the volume transition behaviours. When the nonionic NIPAAm hydrogel is dried before placed in the aqueous ethanol solution, a single phase transition occurs when the ethanol concentration increases, whereas three phase transitions are observed 1.2 Historical Development of Modelling Hydrogel 23 when the hydrogel is immersed directly in the aqueous solution without drying process (Huther et al., 2002). Washing the prepared hydrogels results in a considerable reduction of volume transition of the NIPAAm/sodium methacrylate hydrogels in aqueous ethanol solutions, which is ascribed to the exchange of hydrogen ions with sodium ions and the conversion of completely dissociated sodium methacrylate groups into weakly dissociated methacrylic acid groups (Huther et al., 2002). Electrolytes Addition of electrolyte in the medium of volume transition of the hydrogels may alter the interactions of polymer–polymer, polymer–water, polymer–ion and water– ion. The addition of salt ions may enhance the polymer–water mixing conditions (salting-in) to enhance the volume transition or may impair the conditions (saltingout) to suppress the volume transition. It is observed that the salts of bromide and chloride exert the salt-out effect, whereas the iodide produces the salting-in effect on the volume transition of the copolymeric hydrogels of N-acryloyl-N -alkyl piperazine and MMA (Gan et al., 2001). Usually the cations exhibit the salting-out effect and the volume transition decreases in the well-known Hofmeister order (Muta et al., 2001c). The decrease of degree of the volume transition of the hydrogels in aqueous salt solution is dependent on the counterion species, irrespective of the co-ions (Atta, 2002). However, the relative order of cations may reverse with different anions due to ion pair effects. The Hofmeister order for anions is also observed in the salting-out property. For example, the order of effectiveness in the depression of the degree of the volume transition of the HEMA/PEG hydrogel in aqueous salt solutions follows the sequence Cl− > Br− > I− (Bajpai and Shrivastava, 2002a, b, c). The Hofmeister order demonstrates the promotion of hydrophobic associations that arise from the alteration of water structure and thus the free energy of interaction between polymer and water. The low-frequency Raman scattering experiments reveal that the presence of alkali metal chloride salts tends to reduce the chemical potential of water, which causes the exclusion of water molecules from the NIPAAm hydrogel network chains, probably the proximity of isopropyl groups (Annaka et al., 2002). The Hofmeister order shows that Cit3− is the water structure breakers, whereas SCN− is the water structure maker. Therefore, Cit3− efficiently suppresses the volume transition of poly(NIPAAm-co-dimethylaminoethyl methacrylate) hydrogel, whereas SCN slightly increases the swelling in the concentration range from 10−5 to 10−3 M (Zha et al., 2002). The salt ions may change the electrostatic interactions within the hydrogels. They may shield the ionized groups attached onto the polymeric network chains and screen the ion pair interactions. Shielding of ionized 16-acryloylhexadecanoic acid (AHA) groups results in the disorder−order transition of poly(AHA-co-AAc) hydrogel (Matsuda et al., 2000). The shielding effect caused by the counterions drastically decreases the swelling of poly(MAAc) in NaCl solution when the ionic strength increases (Zhang and Peppas, 2000). Screening of the intra-chain and intra-group interactions within the poly(1-(3-sulfopropyl)-2-vinyl-pyridinumbetaine) hydrogel remarkably increases the swelling of the hydrogel in dilute 24 1 Introduction aqueous salt solution (Xue et al., 2001). In particular, the anti-polyelectrolyte behaviour of the amphoteric hydrogels is observed in poly(N-vinylimidazole-cosodium styrene sulfonate) hydrogels (Valencia and Pierola, 2001). The swelling ratio increases slightly upon increasing the ionic strength of the aqueous salt solution. This is due to the reduction of intra-group and intra-chain aggregations of zwitterionic monomer units by the external electrolytes. The electrostatic interaction in electrolyte solution significantly changes the swelling behaviour of the smart hydrogel subject to externally applied electric field due to the movement of the ions towards their counter-electrodes. The increase of NaCl concentration enlarges the bending angle of the PVA/chitosan IPN hydrogel under electric field (Kim et al., 2002). It is noted that the PVA/poly(diallyldimethylammonium chloride) IPN hydrogel performs the largest bending angle in 0.2 wt% NaCl aqueous solution (Kim et al., 2003a, b), which may be attributed to the coupled effect of increasing free ion movement from the surrounding solution towards their counterelectrodes or into the hydrogel and the shielding effect of the poly-ions by the ions in the electrolytic solution. Ion-specific interactions with hydrophobic sites of the hydrogels complicate the salt influences on the swelling of hydrogels. The vibrational Raman spectroscope study reveals that the addition of lithium perchlorate into poly(AAm) hydrogel strongly disturbs the hydrogen bonding of both the polymer network and the interstitial water due to the specific interaction of lithium with amide groups and causes the structural breakdown by the perchlorate anions (da Costa and Amado, 2000). The amide groups become more accessible to chemical transformations and the hydrogel flexibility increases. It is known that a specific divalent−polymer interaction reduces the effective charge per poly(AAc) polymeric chain at various degrees and the interaction seems to be related to the energy of hydration of the cations (Boisvert et al., 2002). The ion−polymer binding increases with increasing the electrolyte concentration, which leads to the increase of hydrophilicity and thus the degree of swelling of the hydrogels (Lobo et al., 2001). However, the further increase of salt concentration beyond an optimum binding of the ions with polymer chains might reduce the volume transition of the hydrogel (Bajpai and Shrivastava, 2000). In the presence of the thiocyanate ions (CNS− ) in the concentration range from 0.01 to 0.40 M, the swelling ratio of the poly(HEMA)/PEG IPN hydrogels increases with increasing the salt concentration due to the formation of the thiocyanate−polymer complexes. The polymer-bound thiocyanate ions render the hydrogels negatively charged (Bajpai and Shrivastava, 2002). Formation of electrolyte−polymer complexes decreases the swelling degree of the poly(N-vinyl-2-pyrrolidone/itaconic acid) hydrogels due to the exclusion of water molecules by adsorbed electrolytes in the hydrogel system (Sen and Güven, 2002). Ionic osmotic pressure can be used to quantify the salt effect without ion-specific interactions. In general, the increase of ionic strength decreases the osmotic pressure since the higher salt concentration reduces the concentration gradient between the inside and the outside of hydrogels. The greater size the diffusible ion has, the lesser osmotic pressure difference occurs between the interior hydrogel and the external solution, consequently, the lesser volume transition the hydrogel behaves. For halide 1.2 Historical Development of Modelling Hydrogel 25 anions, the sequence in the increasing order of ion sizes is Cl− <Br− <I− . The same order of the degree of the volume transition is observed in the poly(AAc-styrene) hydrogels in potassium halide solution with concentrations ranging from 0.01 to 0.1 M (Bajpai and Shrivastava, 2001). Crosslinkers and Crosslink Density The structure and elasticity of the hydrogels depend on the nature of crosslinking agent as well as on the crosslinking degree. The crosslinking density is the critical indicative parameter that controls the volume transition behaviours and mechanical properties of the smart hydrogels. The osmotic pressure of the crosslinked polymeric network can differ from that of the non-crosslinked one with the same chemical nature. Different crosslinking methods can distinctly influence the prepared polymer network structure and subsequent volume transition behaviours (Martens and Anseth, 2000). Crosslinking by γ-ray irradiation randomly introduces the crosslinks in the hydrogels, whereas the chemically crosslinked hydrogels exhibit more inhomogeneous distribution of crosslinking points due to the difference in the reactivity ratios of monomers and crosslinkers (Pradas et al., 2001). The inhomogeneity of the chemically crosslinked hydrogels increases with increasing crosslinker concentration due to the diffusive nature of the conventional polymerization reaction. The small angle neutron scattering studies demonstrate that the poly(NIPPAm) hydrogels crosslinked by γ-ray irradiation are more homogeneous than the hydrogels crosslinked by conventional polymerization with BIS (Norisuye et al., 2002). The differences of the hydrogel structures can be interpreted well by the statistical-mechanical Panyukov−Rabin theory (Panyukov and Rabin, 1996). The structure of the hydrogels is also determined by the functionality and hydrophilicity of crosslinkers. Hexafunctional crosslinkers generate more rigidly crosslinked polymer networks, compared with tetrafunctional crosslinkers. Therefore, it greatly reduces the volume transition of hydrogels when the tetrafunctional crosslinker is replaced by the hexafunctional crosslinker (Karadag and Saraydin, 2002). When a hydrophilic crosslinking agent is employed, the hydrogel behaves a high affinity towards the aqueous solution owing to the presence of polar groups (Castelli et al., 2000). The degree of the volume transition of hydrogels increases with increasing the polarity of the polar groups in the hydrophilic crosslinker (Martens and Anseth, 2000). By replacing bisacrylamide with more hydrophilic glyoxal bis(diallyacetal) (GLY) as crosslinker, the swelling of the crosslinked poly(NIPAAm) hydrogel is enhanced (Xue et al., 2001; Xue and Hamley, 2002). The pronounced increase of the polymer−water interaction parameter is also observed with increasing GLY content. The swelling degree of the hydrogel is reduced obviously as the amount of crosslinker increases. The degree of swelling is observed to decrease with the crosslink density at exponent of 0.5 (Alvarez-Lorenzo and Concheiro, 2002). However, at low crosslink density, the increase of amount of hydrophilic crosslinker may increase the degree of swelling. The poly(HEMA) hydrogels show an exceptionally large increase of swelling with increasing the amount of crosslinker 26 1 Introduction tripropyleneglycol diacrylate at pH 12.0 (Ferreira et al., 2000). Hydrolysis of HEMA or tripropyleneglycol diacrylate in the highly crosslinked hydrogels is supposed to contribute to the enhancement of swelling. Surfactants The interaction between the hydrogel and surfactant is of great importance for understanding the fundamentals of the volume transition of hydrogels because of the amphoteric property of surfactants. The hydrogels can be ionized upon binding of ionic surfactant molecules to the polymer network through hydrophobic interactions. The polymer−surfactant complex is formed when the surfactant is above the critical aggregation concentration (cac) (Gan et al., 2001). In general, cac is lower than the critical micelle concentration (cmc) of the respective surfactant. The charged head groups of the surfactant molecules bound to the polymer chains give rise to the electrostatic repulsion among the polymer chains, which results in the increase of the volume transition and the lower critical solution temperature (LCST) of the hydrogels. The addition of sodium dodecyl sulfate (SDS) at concentration up to 0.5 wt% causes the significant increase of the swelling ratio of NIPAAm/DPAM copolymeric hydrogel and the LCST value (Xue and Hamley, 2002). When the SDS concentration exceeds 0.5 wt%, there are two volume phase transitions at 36–40 and 70◦ C, respectively. However, the cationic surfactant in very dilute solution behaves like simple electrolyte and exerts salting-out effect on the hydrogels, hence the LCST values decrease initially (Gan et al., 2001). Solvents Addition of other solvents into water may affect the conformation of the hydrogels and the hydrogen bonding between the hydrogels and water (Tokuhiro, 2001), which changes the interactions of polymer–polymer, polymer–solvent, water–solvent and solvent–solvent. Depending on acetone concentration, two transition regions with different swelling ratios are observed due to formation of a two-phase structure (Ilavsky et al., 2002). When the dimethylsulfoxide (DMSO) content in the DMSO–water mixtures is continuously increased, the poly(TBA-co-AAm) hydrogel exhibits the reentrant volume transition behaviour (Ozturk and Okay, 2002). The poly(TBA-co-AAm) hydrogel also exhibits the reentrant conformational transition in the ethanol–water mixtures (Ozmen and Okay, 2003). When the alcohol concentration is increased from 0 to 100 vol%, the poly(acryloyl-l-proline methyl ester) hydrogels show the two swelling phases, the first swelling at 0–10 vol% and the second swelling at 50–80 vol%, and the two shrinking phases, the first shrinking at 10–50 vol% and the second shrinking at 80–100 vol%, in all the aqueous alcohol solutions (Hiroki et al., 2001). The reentrant phase transition of the poly(NIPAAm) hydrogels is also observed in the polymeric solvent PEG and water mixture (Melekaslan and Okay, 2001). The competing attractive interactions between water–solvent and polymer–solvent are responsible to the reentrant phase transition. 1.2 Historical Development of Modelling Hydrogel 27 Addition of polymeric solvent into the medium may selectively increase the external osmotic pressure and consequently decrease the volume transition of the hydrogel, which is observed in the swelling of the NIPAAm hydrogel in aqueous PEG solution (Huther et al., 2002). The degree of swelling of the hydrogel decreases with increasing the PEG concentration in solution, and a phase transition to a shrunken state occurs. The swelling of the Na-gel in HPC solution decreases (Evmenenko and Budtova, 2000). Unlike the organic solvents, the polymeric solvents may form complexes with the polymer network, and thus change the volume transition behaviours of the hydrogels. The formation of complex between HPC and poly(AAc) hydrogel decreases the swelling of the poly(AAc) hydrogel with the increase of HPC concentration in aqueous solution (Evmenenko and Budtova, 2000). Co-nonsolvency effect is observed upon addition of any solvent to the poly(NIPAAm)–water system (Costa and Freitas, 2002). Co-nonsolvency is referred to poor solubility in mixture of solvents that are good solvents individually for the polymer. In a general manner, the poly(NIPAAm) solubility is reduced within the range of intermediate solvent concentrations in binary aqueous solutions due to the preferential hydrophobic hydration of solvent molecules in water-rich region, which results in the weakening of the poly(NIPAAm)–water interactions. Metal Ions Unlike simple cations, heavy metal ions have strong affinity to polar groups. Addition of metal ions may decrease the swelling of the hydrogel (Katime and Rodriguez, 2001; Vashuk et al., 2001). The adsorption of heavy metal ions by the hydrogels leads to more physical crosslinking formed by the inter-chain metal complex formation (Loh et al., 2001). However, the capacity of metal adsorption decreases with increasing the crosslinker density due to the more rigid polymer networks. The metal binding in ionic poly(MAAc-co-AAc) hydrogels is proposed to be entropy driven (Eichenbaum et al., 2000). Therefore, there is a distinct difference of the metal ion binding affinity between ionic hydrogels. Hydrogen Bonding Effect Hydrogen bonding effect has significant influence on the volume transition behaviours of the hydrogels in water, where water forms strong hydrogen bonding with hydrophilic polymer chains (Qu et al., 2000). The mechanism of the volume transition behaviours of the hydrogel is partially controlled by rearrangement of hydrogen bonding. The AMPS/N-t-butylacrylamide hydrogel performs a discontinuous phenomenon of volume transition as the hydrophilic–hydrophobic balance is changed (Varghese et al., 2000), because of the alteration of the hydrogen bonding in the hydrogel–water system and temperature-dependent hydrophobicity of the polymer. Formation of hydrogen bonding makes the hydrogel more hydrophobic, which leads the hydrogel to a collapsed state, which is observed in the poly(MAAc-co-methacryloxyethyl glucoside) hydrogels in acidic media (Kim 28 1 Introduction and Peppas, 2002). Deswelling of the poly(MAAc) hydrogel is the result of the hydrogen bonding formation arising from the protonation of the carboxylic acid groups. The hydrogen bonding increases with the MAAc content in the copolymer networks. Intermolecular hydrogen bonding intermediated by water molecules is also found to play an important role in the mechanism of deswelling of the poly(N-vinyl-2-pyrrolidone) (PVP) hydrogels (Muta et al., 2002). On the other hand, the destruction of hydrogen bonding may increase the hydrophilicity of the system and thus increase the degree of swelling. The dissociation of the hydrogen bonding between the chitosan and PEO as well as the ionization of the amine functions in the chitosan–PEO semi-IPN hydrogels leads to the relaxation of the macromolecular chains when pH is in acidic condition (Khalid et al., 2002). The ionic hydration can stabilize or destabilize the hydrogen bonding network (Muta et al., 2001a, b). The hydrogen bonding of water in the hydrogels is strengthened in the presence of strongly hydrated cations or weakened in the presence of strongly hydrated anions (Muta et al., 2001c). Integrating hydrophobic groups to the hydrogels decreases the hydrogen bonding of water in the hydrogels (Yasunaga et al., 2002). Water State In general, water in the hydrogels exists in three physical states: (1) the free water which can freeze at the usual freezing point, (2) the intermediate water which is less strongly associated due to the existing hydrophobic interactions and can freeze at a temperature lower than the usual freezing point and (3) the bound water which is strongly associated with the hydrophilic segments of hydrogels and cannot freeze at the usual freezing point (Dibbern-brunelli and Atvars, 2000; Li et al., 2000; Ito et al., 2000; McConville and Pope 2001; Manetti et al., 2002; Meakin et al., 2003). The swelling characteristics of the hydrogels are dominated by the nature of the polymer and the state of water. The poly(N-vinyl 2-pyrrolidone-graft-citric acid) hydrogels exhibit continuous changes in water content as a function of temperature, which is attributed to the fact that water remaining within the hydrogels consists mostly of the binding water (Caykara et al., 2000). The oscillation in volume transition behaviour is related at least to the three types of water molecule movement in the hydrogels (Makino et al., 2000). The content of non-freezing water is affected by the chain mobility or crosslink density of the hydrogels. Various hydrogels are reported to have quite different contents of non-freezing water, for example, the 23% non-freezing water in the chitosan–PEO hydrogel (Khalid et al., 2002), the 24–28% non-freezing water in a chitosan hydrogel (Qu et al., 2000), the 35% non-freezing water in the HEMA hydrogels and as high as the 43% non-freezing water in the 2,3-dihydroxypropyl methacrylate (DHPMA) hydrogels (Gates et al., 2003). The molecules of nonfreezing water are hydrogen bonded to the hydrophilic groups of the hydrogels. Therefore, the content of non-freezing water is proportional to the amount of hydrophilic groups in the hydrogels. The content of non-freezing water increases 1.2 Historical Development of Modelling Hydrogel 29 with the increase of the ratio of hydrophilic groups (Katime and de Apodaca, 2000) and decreases with the increase of the ratio of hydrophobic groups (Kim et al., 2003). Obviously, the proportion of free water becomes preponderant as the swelling ratio increases. 1.2.2 Transient Modelling for Kinetics of Smart Hydrogels The present transient models focus on the responsive kinetics of the smart hydrogels subject to different environmental stimuli, especially in the rates of swelling or shrinking process of fast response hydrogels. Currently the fast response hydrogels are increasingly attracting attention. Usually their fast response can be achieved in five ways: (1) reducing the dimension of the hydrogels due to the swelling rate being inversely proportional to the square of the geometrical size of the hydrogels; (2) forming the heterogeneous network structure by phase separation technique; (3) introducing the porosity into the hydrogels; (4) graft copolymerization where the free ends of the grafts act to accelerate the dehydration rate and (5) using the silane crosslinking agent. The extensively studied phase separation technique is an approach for preparation of the fast response hydrogel. The poly(N-isopropylacrylamide-co-methyl methacrylate) hydrogels with capability of fast response can be prepared through the phase separation technique in water/glacial acetic acid as the mixed solvent (Zhang and Zhuo, 2002). Using water/acetone as the mixed solvent during the redox polymerization/crosslinking reaction, the fast responsive poly(N-isopropylacrylamide) hydrogel may also be prepared (Zhang and Zhuo, 2000a). This is attributed to the fact that the polymer chains produced in the mixed solvent are very soluble and get widely expanded during polymerization. Owing to the widely expanded chains, the polymer system is more unstable, and thus it exhibits the fast deswelling rate. The electron beam irradiation provides another technique for phase separation. The thermo-sensitive poly(N-isopropylacrylamide) hydrogels crosslinked by electron beam irradiation are prepared (Panda et al., 2000), which shrink about 100 times faster than the conventionally crosslinked gels. The mechanism of the fast response of the hydrogels may be attributed to the two effects: (1) the polymerization and crosslinking at extremely high dose rates may result in intra-molecularly crosslinked gels and (2) the temperature during electron beam irradiation may rise above the lower critical solution temperature (LCST), resulting in the phase separation in polymerization during crosslinking reaction. In addition, it is noted that the porous structure enlarges the surface area to volume ratio and allows the solute to diffuse more rapidly into the hydrogel. The porous hydrogels may be made by several methods, such as the porogen leaching, phase separation, particulate crosslinking, microemulsions, gas blowing and freeze drying. Addition of polyethyleneglycol (PEG)-400 as the pore-forming agent to the monomer solution of N-isopropylacrylamide (NIPAAm) is found to dramatically increase the swelling kinetics of the prepared hydrogels (Zhang and Zhuo, 2000b). The higher the PEG-400 contents are in the monomer solution, the larger fraction the big pore sizes are in the network of the hydrogel. 30 1 Introduction R By adding a gas-forming agent Pluronic F127 during polymerization, the superporous sucrose hydrogels are synthesized (Chen and Park, 2000). Compared with the sucrogels, the superporous hydrogels swell faster with higher ratio of swelling and degrade faster in both acidic and basic conditions. The gas blowing technique is also employed to prepare the superporous poly(acrylamide-co-acrylic acid) hydrogels whose response is the orders of magnitude faster than that expected for nonporous hydrogels with the same dimension (Gemeinhart et al., 2000). The superporous hydrogels have low bulk density of 0.30±0.03 g/ml and water molecules are taken up into the superporous hydrogels by capillary forces. By reducing the dimension of the hydrogels as well as introducing the porous structure into the hydrogels, the fast pH- and ionic strength-sensitive hydrogels are prepared in microchannels by photopolymerization of monomer mixtures containing water and surfactant (Zhao and Moore, 2001). The mechanism of the fast response of the hydrogels is attributed to the porous structure generated by the surfactant phase template and phase separation, irrespective of the network crosslinking density or acrylic acid (AAc) composition in the hydrogel. The swelling of the hydrogels follows the second order of kinetics (Quintana et al., 1999). A two-step polymerization method is proposed to prepare the fast response thermo-sensitive poly(NIPAAm-co-di-npropylacrylamide) hydrogels (Xue and Hamley, 2002), where the polymerization is conducted at 20◦ C for a short time and the polymerization is then completed at −28◦ C. The responsive kinetics can be adjusted according to the polymerization time at 20◦ C, which seems to influence the porosity of the network structure of the hydrogels. The literature search reveals that the transient models for simulation of kinetics of the smart hydrogels have so far been limited probably due to the limited experimental data. The fast response hydrogels have found wide-range promising applications in various areas, such as the mechano-chemical actuator and sensor, drug delivery device and especially in the bio-micro-electro-mechanical system (BioMEMS), as well as biomaterials for biomedical and tissue engineering applications. The ready mathematical models with capability of predicting and simulating the responsive kinetics of the fast response smart hydrogels are undoubtedly crucial for the applications. The fast response hydrogels provide an attractive routine to investigate the kinetics of volume variation. Currently the modelling development of the volume variation of the fast response hydrogels is becoming a popular research area. A review on the developed models could greatly facilitate this effort. In this section, three typical models developed with different complexities are discussed to investigate the kinetics of the volume variation of the hydrogels. A phenomenal model based on the second order of reaction kinetics provides a simple method to correlate the experimental data of kinetics. A power law model can be employed to evaluate different mechanisms of the volume variation according to the diffusion exponential coefficients. The multi-field model couples the mechanical deformation with the diffusion of ion species. The rate of volume variation is dependent on both hydrogel molecular design and operation conditions. Several key parameters are summarized for simulation of kinetics of the fast response smart hydrogels. 1.2 Historical Development of Modelling Hydrogel 31 220.127.116.11 Mathematical Models and Simulations The kinetics process of swelling of the smart hydrogels is a complicated phenomenon, which generally involves three successive steps: (1) the diffusion of water molecules into the polymer system; (2) the relaxation of the hydrated polymer chains and (3) the expansion of the polymer network in surrounding aqueous solution. The swelling kinetics of the hydrogel may be further divided into more detailed steps. For example, the kinetics process of the swelling or shrinking of poly(N-vinylimidazole-co-sodium styrene sulfonate) hydrogels includes the following simultaneous steps (Valencia and Pierola, 2002): (1) the diffusion of water towards the hydrogel; (2) the chain disentanglement; (3) the sodium–proton interchange through the external bath boundary; (4) approaching of chains to allow the interaction of sulfonate groups with neighbouring protonated imidazole moieties and (5) the diffusion of water outside the hydrogel. On the other hand, the wetting process of polymer dry gel with cylindrical shape is divided into three steps (Ji and Ding, 2002): (1) swelling of the gel in the radial direction with cusp-like patterns evolving on the surface; (2) shrinking of the gel in the radial direction and swelling in the axial direction and (3) the re-swelling of the gel to the final stage and eventually disappearing of patterns. Generally, two processes are employed to describe the diffusion of water into the polymer matrix, namely the diffusion of the solvent into the swollen matrix and the advancement of the swollen–unswollen boundary as a result of polymer relaxation. When the rate-determining step is the diffusion of the solvent into the swollen matrix, there is a linear relation between the water uptake and time1/2 , the system is regarded to exhibit the Fickian behaviour. In contrast, if the advancement of the swollen–unswollen boundary is slower than the diffusion of the solvent in the swollen polymer, the zero order of kinetics is achieved with the water uptake time, and the system is regarded to exhibit the non-Fickian behaviour. In pure water condition, the diffusion of water generally approaches to the Fickian behaviour. However, the diffusion of water into the hydrogels under solution conditions follows the non-Fickian behaviour due to the dominance of polymer relaxation. The swelling of the poly(NIPAAm) hydrogel in the gelated corn starch aqueous solution is determined mainly by the relation of hydrated polymer chains, instead of the water diffusion rate (Zhang and Zhuo, 2000c). The starch may act as the long graft-like chains of the poly(NIPAAm) hydrogels, which provides the channels for water to be released during the shrinking process. It is claimed that the molecular relaxation controls the velocity of water uptake of hydroxypropylmethyl cellulose (HPMC), carboxymethylcellulose-sodium (NaCMC) and mixed HPMC/NaCMC hydrogels irrespective of pH of the aqueous phase (Michailova et al., 2000), in which there is an inversely proportional dependence between the viscosity and the water uptake velocity. Three typical transient models developed with different complexities are reviewed here for simulation of the kinetics of the volume variation of the smart hydrogels. They are the phenomenal model, the power law model and the multi-component diffusion model. 32 1 Introduction Phenomenal Model The phenomenal model is based on experimental observation for describing the extensive polymer swelling (Schott, 1992) and is written as follows: t = A + Bt W (1.34) where W is the water uptake at time t, B= 1/W∞ is the inverse of the maximum swelling W∞ and A = 1/(dW/dt)0 is the reciprocal of the initial swelling rate. Equation (1.34) implies the second order of kinetics of swelling for volume variation of the hydrogels, which is expressed as dW/dt = kr (W∞ − W)2 . The specific 2 ). By substituting rate kr is a constant related to the parameter A as kr = 1/(AW∞ the swelling data into Eq. (1.34), it is found that the plots of t/W against t can give straight lines with good correlation coefficients for experimental observations. Obviously, the phenomenal model cannot provide accurate information about the mechanism of the volume variation of hydrogel. In most cases, the initial phase of the volume variation of hydrogel follows the zero order of kinetics of swelling, instead of the second order of kinetics. This means that the model is suitable for simulation of kinetics of the hydrogel volume variation after the initially fast swelling process. However, at least it provides a simple approach to correlate experimental data. Power Law Model As well known, the diffusion of water into the hydrogel system results in the volume variation of the hydrogels. The water transport in the hydrogels can be characterized either by Fick’s second law or by a more advanced equation of anomalous diffusion, which incorporates a diffusive term coupled with a pseudo-convective velocity term. A simple method of describing water transport in polymers is given via the power law (Astarita, 1989) Mt /M∞ = ktn (1.35) where Mt is the mass of water gained or lost at time t, M∞ is the initial mass of water contained in the polymer, k is a constant and n is the diffusion exponent. Usually the mechanism of the water transport in the hydrogels may be characterized by the diffusion exponent n and also by two limited cases of this power law model, n = 0.5 and n = 1. When n = 0.5, the water transport is controlled exclusively by the chemical potential gradient, little or no volume variation occurs during the transport. This is referred to as Case I diffusion or Fickian diffusion, and then the volume variation can be described by a diffusion coefficient. If n = 1, the rate of the volume variation of the hydrogels is proportional to time t, in which the stress relaxation controls the kinetics of the volume variation of the hydrogels and the volume variation counteracts the mechanical stresses produced by water transport. This 1.2 Historical Development of Modelling Hydrogel 33 is termed Case II diffusion, where the velocity of the waterfront describes the kinetics process of the volume variation. The intermediate case called the anomalous diffusion occurs when the water transport is proportional to tn , where 0.5<n<1. Actually the water transport in the hydrogels may result from a mixture of Case I and Case II processes, in which both the waterfront velocity and diffusion coefficient are required to characterize the volume variation process (Chou et al., 2000). A model proposed can account for Case I, Case II and anomalous water transport processes (Harmon et al., 1987), in which the total flux J consists of two components, One is due to the diffusion with a concentration gradient and the other is due to the stress relaxation of polymer chains with a propagation speed v. For example, for one-dimensional volume variation of the hydrogels J = −D ∂C + v(C − C0 ) for ∂X 0 ≤ |X| ≤ 1 (1.36) where C = C(X) and C0 = C(0) are the concentrations at points X and X = 0, respectively. The diffusion coefficient D and the velocity v come from Case I and Case II water transport processes. According to the law of mass conservation, one can have ∂ 2C ∂C ∂C =D 2 −v ∂t ∂X ∂X for 0 ≤ |X| ≤ 1 (1.37) After integrating the concentration over the domain with the boundary condition of constant surface concentration C0 at X = ±1, the variation of water mass Mt at time t associated with the equilibrium water mass M∞ is written as follows (Harmon et al. 1987): Mt =1−2 M∞ ∞ n=1 vl λ2n 1 − 2 cos λn exp − 2D βn2 Dt exp − 2 l 2 βn4 1 − 2D vl cos λn (1.38) where vl tan λn 2D v2 l2 + λ2n βn2 = 4D2 λn = (1.39) (1.40) where the roots λn (n= 1, 2, 3, ..., ∞) of Eq. (1.39) are used in Eqs. (1.38) and (1.40), respectively. For a special case where v is equal to zero, Eqs. (1.39) and (1.40) are simplified to λn = (n + 1/2)π and β n = λn , respectively. Equation (1.38) is then reduced to ∞ Mt M∞ = 1 − n=1 8 (2n + 1)2 π 2 exp −(2n + 1)2 π 2 Dt l2 (1.41) 34 1 Introduction The short-time limited expression for Eq. (1.41) is thus obtained as Mt = M∞ 4 π 0.5 Dt l2 0.5 (1.42) It is observed from the above equation that the relation between Mt /M∞ and t0.5 yields a straight line. Based on the slope of the graph, the value of diffusion coefficient D is calculated. As a good example of applications, the experiment of the water transport in crosslinked 2-hydroxyethyl methacrylate (HEMA) hydrogels is in excellent agreement with the prediction by the model (Chou et al., 2000). In order to achieve better approximation, the exact solution of Eq. (1.37) is derived, termed the Berens–Hopfenberg model (Enscore et al., 1977; Berens and Hopfenberg, 1978), and it is expressed as follows: n=∞ Mt M∞ = φF 1 − n=1 −D (2n + 1)2 t 8 exp 4 l2 (2n + 1) π 2 (1.43) +φR (1 − exp (−kt)) where k is the first order of relaxation constant, øF and øR are the fractions of water uptake contributed by the Fickian diffusion and the chain relaxation, respectively. This heuristic model can be used for analysis of the overall water uptake in terms of the Fickian and non-Fickian contributions, which leads to the determination of both the diffusion coefficient D and the characteristic relaxation time τ that is defined as the reciprocal of the constant k. It is noted that the model mentioned above does not take into account the interactions between the polymer and the solvent, which significantly influence the water diffusion and the stress relaxation of polymer chains. In addition, the diffusion coefficient D is assumed to be constant in the model. In fact, the hydrogel network structure always changes with the volume variation of the hydrogel, which results in a varying diffusion coefficient. However, at least when 0 < Mt M∞ < 0.60, the model can predict well the kinetics process of volume variation of the smart hydrogels. Multi-field Model The kinetics of the volume variation of the hydrogels involves the water diffusion and the mechanical deformation simultaneously. For the ionic hydrogels, the volume variation of the hydrogels is strongly dependent upon the diffusions of all species and the variation of electrical potential. A good model for the volume variation of the hydrogels should be able to incorporate the multi-field effects. Modelling of the ion transport could be conducted by many models within various theoretical frameworks. It is sufficient to model the ion transport as follows: ∂ ∂ cZk FDk ∂φ ∂ck ∂ck = Dk + ∂t ∂x ∂x ∂x RT ∂x (1.44) 1.2 Historical Development of Modelling Hydrogel 35 where ck is the concentration of the ion species k, Dk is the binary diffusion coefficient of the ion species k, c is the total concentration, zk is the valence of the ion species k, ø is the electrostatic potential, F is the Faraday constant, R is the universal gas constant and T is the absolute temperature. The concentration of ionized pendant groups in the polymer network is always in equilibrium with the concentration of hydrogen ions in the polymer network. The kinetics of swelling of the ionic hydrogels induced by pH change is modelled by considering the diffusion of hydrogen ions, which is governed by the chemical diffusion equation together with the mechanical equation (Chatterjee et al., 2003). This model assumes that the mechanical deformation of the polymer network occurs instantaneously with the diffusion of hydrogen ions. The mechanical equation takes into account the deformation of the polymer network that occurs during the diffusion of hydrogen ions into the hydrogel, namely k = φ −Dk ∂ck ∂ψ − μk zk ck + ck U ∂x ∂x (1.45) where k is the flux of the kth ion, ø is the gel porosity and U is the area-averaged fluid velocity relative to the polymer network. The diffusion rate inside the hydrogel is related to the diffusion in aqueous solution through the obstruction model as follows: 2 Dk K = (1.46) Dk 2+H where H is the hydration of the hydrogel and it is defined as the ratio of fluid volume to polymer volume. Continuity condition for the divergence of each ionic flux is given by ∂ (αk ) ∂ HCk + Hcbk = − (1.47) ∂t ∂X where cbk is the concentration of the ion k that can be reversibly bound to the polymeric fixed charge, X is the Lagrangian coordinate system associated with the hydrogel and α is the total hydrogel area normalized to its initial area. The concentration of the ion k reversibly bound to the polymeric chains (cbk ) in the presence of chemical reactions is calculated by (Grimshaw et al., 1990) cbk = c0f ck H (K + ck ) (1.48) where c0f is the total concentration of ionizable groups within the hydrogel before the volume variation. By rearrangement of the above equations, a nonlinear diffusion–reaction equation for the concentration of H+ ions in the hydrogel is obtained as c0f ∂ ∂cH ∂ψ ∂ αφ DH −αcH U (1.49) =− cH H + + μH zH cH ∂t K + cH ∂X ∂x ∂x 36 1 Introduction where D̄H is the diffusion rate of hydrogen ions within the hydrogel, cH is the internal concentration of hydrogen ions and cbH is the concentration of hydrogen ions reversibly bound to the fixed charges of the hydrogel. The presence of buffer in the solution increases the apparent diffusion rate of hydrogen by providing an alternate path for diffusing hydrogen ions between the hydrogel and bath solution. Buffer augmented transport of hydrogen ions under certain conditions may result in the apparent diffusion rates of hydrogen, which is several orders of magnitude higher than the diffusion coefficient of hydrogel alone (Ohs et al., 2001). It is found that the kinetics of the water uptake in the buffered solutions is markedly faster than that in the unbuffered solutions for the hydrophobic ionizable copolymer gels composed of PEG, AAc and styrene, though the water uptake is contributed by both the mechanisms of diffusion and polymer chain relaxation (Bajpai and Shrivastava, 2001). The influence of the buffer on the transport of hydrogen ions can be modelled by including additional terms in the continuity equation of hydrogen ions within the hydrogel ∂(αH + αHB ) ∂ HcH + HcbH + HcHB = − ∂t ∂X (1.50) where cHB is the concentration of hydrogen ions bound to the buffer, H is the flux of hydrogen ions and HB is the flux of hydrogen ions bound to the buffer. cHB = cT cH (KB + cH ) (1.51) where KB is the dissociation constant of the buffer and cT is the total buffer concentration. The flux of the buffer is proportional to the flux of the hydrogen ions: HB = DHB DH cT KB + cH H (1.52) where DHB is the diffusion rate of buffer in the hydrogel. The Poisson equation is used to calculate the electrostatic potential F ∂ 2ψ =− 2 εε0 ∂x N zk ck + zf cf (1.53) k=1 The chemical diffusion equation then becomes c0f cH ∂ HcT cH + HcH + ∂t K + cH KB + cH H ∂ DHB cT ∂cH α 1+ =− DH ∂X 1+H ∂x DH KB + cH (1.54) 1.2 Historical Development of Modelling Hydrogel 37 The change in the hydration of the hydrogel is calculated by the following mechanical equation that describes the forces and fluid flow: ∂H ∂ ak = ∂t ∂X ∂ (Mε) ∂ψ − + zf cf F ∂x ∂x (1.55) where k is the hydraulic permeability of the hydrogel, M is the bulk modulus of the hydrogel and ε is the compressive strain. The advantage of this model is the capability of providing a good evaluation of the volume variation of the hydrogel by integration of the chemical, electrical and mechanical interactions. It captures the variations of the concentration distributions of all ionic species with time. However, this model is valid only for the ionic hydrogels, and the deformation of the polymeric network matrix is characterized by the volume-based hydration H, instead of the displacement vectors. The mathematical complexity also limits its extensive applications. 18.104.22.168 Key Parameters in Transient Modelling for Kinetics of Hydrogels Although there are many parameters having influences on the kinetics of volume variation of the smart hydrogels, basically they may be classified into two categories: (1) the designs of the hydrogels, which include the ionic group content, thickness, shape and strength and (2) the operating conditions, which include the intensity and function of environmental stimuli and the type and concentration of ionic species in outer electrolyte solution. A good transient model should be able to characterize the effects of various parameters that have significant influences on the kinetics of volume transition of the smart hydrogel. This is a challenge for modelling development and simulation. Several key parameters are summarized below. Environmental Medium The environmental medium of the hydrogels plays an important role in kinetics of the hydrogels with volume variation. The temperature and pH of solutions are the most widely studied parameters of operation conditions. It is found that, with increasing temperature, the full interpenetrating polymer networks (IPNs) of crosslinked gelation with polyacrylamide experiences an anomalous type of diffusion and the rate of swelling increases with the rise in ambient temperature (Rathna and Chatterji, 2001). For the gelation with poly(NIPAAm) above its LCST, the diffusion deviates from the anomalous to Fickian types, due to the predominance of the hydrophobic characteristics of NIPAAm, resisting the advancing of solvent molecules. The swelling behaviour of thermo-reversible NIPAAm hydrogels is related to their looser or denser structures and pore sizes, which is dependent on the surrounding temperature, polymerization temperature and polymerization media (Lee and Yeh, 2000). However, the effect of solution pH is much more complicated. The kinetics of swelling of poly(N, N -dimethylaminoethyl methacrylate) hydrogels is observed to 38 1 Introduction be the non-Fickian type in lower pH and tend to the Fickian type at higher pH (Chen and Yi, 2001). There is a jump corresponding to the pH values and hysteresis loop on elongation or contraction behaviour for PVA and PAA hydrogels (Fei and Gu, 2002). The elongating process takes place much slower than that of contracting process. Time of swelling to equilibrium for the IPN hydrogels is much longer than that of shrinking to equilibrium (Lu et al., 2000), which is ascribed to the fact that the hydrogels shrink in the skin layer first and form a thick, dense and collapsed skin layer on the surface region. This dense layer is believed to be impermeable to water. Composition of Hydrogels The properties of hydrogels are determined by the composition of comonomers in the hydrogels. It is found that the water sorption by the hydrogels follows both the Fickian and non-Fickian swelling mechanisms, depending upon the composition of the hydrogel (Bajpai and Giri, 2002). The incorporation of hydrophobic comonomers is generally required for fast response of phase transition to pH change. For example, the incorporation of small amount of maleic acid into the nonionic polyacrylamide hydrogels results in the transition of swelling mechanism from the Fickian to non-Fickian swelling behaviours (Bajpai, 2000). Then the hydrogels require more time to swell. The increase of ionic strength causes the decrease of swelling, while the swelling increases with pH of the swelling medium. With lower acid contents, the swelling increases while higher concentrations of maleic acid cause the decrease of swelling. The hydrogels require more time to shrink, compared with that required for swelling. The water uptake of the hydrogel varies sensitively with various contents of the hydrophilic polymer, copolymer, crosslinking agent and the environmental medium temperature (Bajpai and Shrivastava, 2002a–c). The increasing proportion of the hydrophilic polymer PEG results in the shift of the water transport mechanism from the anomalous to Fickian types due to the network with a greater number of macromolecular chains, while the hydrophilic monomer acrylamide tends to move the swelling mechanism from the Fickian to non-Fickian ranges due to the increase of network density. On the other hand, the increasing content of the hydrophobic monomer (styrene) shifts the water-sorption mechanism from the Fickian to anomalous types, which is due to the steric hindrance and dispersion forces operating between the polystyrene chains in the hydrogels. The bending speed increases in proportion to the poly(acrylic acid) content in PVA/PAA semi-interpenetrating network hydrogel (Fei et al., 2002). The increase of the hydrophilicity by acrylic acid (AAc) decreases the response rate to pH variation (Chiu et al., 2001). It is claimed that the swelling ratio and rate increase with increasing the content of the hydrophilic monomer in the hydrogels (Martellini et al., 2002), and there is a significant variation in the diffusion coefficients for different temperatures. The corresponding swelling is classified as Fickian type. It is also observed that, with increasing the PEG content, the value of n increases in the non-Fickian region, while increasing HEMA tends to increase the value of n towards Fickian value in the Fickian range (Bajpai and Shrivastava, 2002a). It is found that the new 1.2 Historical Development of Modelling Hydrogel 39 crosslinked hydrogels based on N-acryloyl-N -methyl piperazine (AcrNMP) and methyl methacrylate (MMA) are able to be responsive to pH and temperature (Gan et al., 2001). With increasing the hydrophilic content in the hydrogels or with rising temperature, the diffusion constants enlarge. The apparent activation energy for the diffusion process is independent of the composition of the hydrogel networks, and the enthalpy of mixing has a strong influence on the hydrophilic content of the hydrogel. It is emphasized that the balance between the two effects, (1) the maintenance of effective hydrophobic aggregation force between collapsing polymer chains and (2) facilitation of water channel formation in the gels to readily release water through the collapsing gel-skin layer, is very important to generate the fast shrinking of NIPAAm and 2-carboxyisopropylacrylamide (CIPAAm) copolymer gels (Ebara et al., 2001). The shrinking rate of NIPAAm–CIPAAm hydrogels increases with increasing CIPAAm content. In contrast, structurally analogue NIPAAm–AAc copolymer gels lose temperature sensitivity with introduction of a few mole percent of AAc. Additionally, the deswelling rates of NIPAAm–AAc gels decrease with increasing AAc content. It is found that the kinetics of swelling of the hydrogels decreases with increasing AAm and MBAAm concentration in the gel matrix (Yildiz et al., 2002). The HEMA-co-sodium acrylate hydrogels may exhibit an overshooting phenomenon in the kinetics of swelling behaviour at higher HEMA content and lower temperature (Lee and Lin, 2001), where the phenomenon that the water uptake of the gel increases over the equilibrium value is called “overshooting”. On the other hand, the presence of impenetrable polymer molecules may lead to the increase of the path length for diffusion, a phenomenon called the obstruction effect. Usually the hydrogel structure changes with the composition. In the study of water permeability in agarose–dextran gels, it is found that the dextran covalently linked to agarose by electron beam irradiation causes very significant reduction in the Darcy permeability, by as much as the order of magnitude (White and Deen, 2002). Modelling and simulation indicate that, at high agarose concentration, the dextran chains behave as fine fibres interspersed among coarse agarose fibrils, whereas the dextran molecules at low concentrations begin to resemble spherical obstacles embedded in agarose gels. Salt Basically salts have significant influences on the kinetics of volume variation of the hydrogels due to the change in the interactions of polymer–polymer, polymer– water, polymer–ion, water–ion and so on. It is observed that the bending speed of the PVA/chitosan IPN hydrogels increases with the increase of the applied voltage and the concentration of aqueous NaCl solution (Kim et al., 2002). However, the time required to reach the equilibrium bending angle depends on the mobility of the cations, the electric field and the gel thickness but not on the salt concentration (Yao and Krause, 2003). In the study of the volume phase transition of poly(NIPAAm) hydrogels induced by aqueous hydroxides and chlorides (Dhara and Chatterji, 2000), the hydrogels 40 1 Introduction exhibit the volume phase transition at additive concentration characteristics of the anion. It is presumed that the bubble formation observed during the anion induced by the deswelling of initially equilibrium swollen gels is the spontaneous separation of the partially collapsed gel into polymer-rich and solvent-rich domains. The permeability of the bubble wall and its stability may be osmotically driven. Crosslink Density The crosslink density directly affects the mechanical deformation of the hydrogels. It is easily understood that the hydrogels with higher crosslink density can have the larger resistance to the deformation during volume variation. The poly(aldehyde guluronate) hydrogels with higher crosslink density show very retarded degradation behaviour (Lee et al., 2000). The rate of hydrogen ion formation is significantly reduced when the crosslinking ratio increases in the gels (Podual et al., 2005). The response rate to the change in external temperature may be improved during the shrinking process and the oscillating shrinking–swelling cycles (Zhang et al., 2003). The interior network structure of the hydrogels becomes more porous with the decrease of the crosslinking level, which provides numerous water channels for the diffusion of water, while the water content decreases with increasing the level of crosslinking at room temperature. It is observed that the increase of N,N methylene bisacrylamide (MBA) concentration enhances the non-Fickian nature of the swelling process, which might be attributed to the slower relaxation of network chains (Bajpai and Shrivastava, 2002b). However, at higher concentration of ethylene glycol dimethacrylate (EGDMA), the equilibrium swelling is attained faster (Bajpai and Shrivastava, 2002a). Diffusion Coefficient Probably the diffusion coefficient has the most important effect on the characteristics of the kinetics of volume variation of the hydrogels. Previous studies utilize the concentration-dependent diffusion coefficient or time-dependent diffusion coefficient or time- and memory-dependent diffusion coefficient. The timeor position-dependent diffusion coefficients are also used to account for the shape change in solvent diffusivity across the swelling front between glassy and rubbery regions in the polymer. The diffusion of water into the polymer matrix may be influenced by the copolymer composition and microstructure that are the features determined by the kinetics of the polymerization of the co-monomers, the polarity of the polymer segment, the glass transition temperature of the polymer, the flexibility of the polymer network, the crosslink density and inter-chain interaction, the molecular weight of the polymer, the degree of chain branching and the presence of bulky co-monomer pendent groups. For example, the diffusion coefficient may be controlled by addition of the non-polar monomers to the polar HEMA monomer. With increasing the proportion of n-butyl methacrylate or cyclohexyl methacrylate in the copolymers with 1.2 Historical Development of Modelling Hydrogel 41 HEMA, the diffusion coefficients decrease, reflecting the influence of the compositional microstructure of the copolymers on the diffusion of water into the cylinders (Hill et al., 2000). The thermal effect dominates at high temperature and the influence of water content is significant at low temperature. The temperature may affect the transport mechanism of swelling of the gels. For example, the diffusion coefficient of the NIPAAm and 1-vinyl-3-(3-sulfopropyl) imidazolium betaine copolymeric gels increases with increasing temperature (Lee and Yeh, 2000). The diffusion coefficients of IPN hydrogels increase with increasing temperature and decrease with increasing the content of poly(propylene glycol) (PPG) (Kim et al., 2003). The diffusion coefficients of water may be concentration dependent. Based on the free volume theory, the relation for the effective water diffusion coefficient Deff with the water concentration cw is written as follows: Deff cw = D0 exp −bi 1 − cw,eq (1.56) where D0 is the limited water diffusion coefficient in the equilibrium swollen hydrogel and cw,eq is the water concentration in the equilibrium swollen hydrogel. Based on the free volume theory suitable for rubbery polymers and considering the plasticization effect induced by the penetrant, a modified free volume model is proposed to predict the diffusion coefficients of small molecule solvent in glassy polymers (Wang et al., 2000). The solvent self-diffusion coefficient at temperature T is expressed as follows: γ (w1 V1∗ + w2 ξ V2∗ E exp − Dself = Dex exp − RT VFH (1.57) The solvent is denoted as component 1 and the polymer as component 2. wi is the mass fraction of component i and Vi∗ represents the specific critical hole-free volume of the component i required for a diffusion jump. Dex is a pre-exponential factor, E is the critical energy that a molecule must possess to overcome the attractive force holding it to its neighbours and γ is an overlap factor that is introduced because the same free volume may be obtained for more than one molecule. ξ is the ratio of the molar volume of the jumping unit of the solvent to that of the polymer. VFH is the average hole-free volume, which is estimated by addition of those for solvent and polymer with the assumption that all volumes associated with the solvent and polymer are additive at any concentration and temperature (Vrentas and Vrentas, 1994). The mutual diffusion coefficient Dm for a solvent–polymer system may be calculated by Dm = D0 (1 − v1 )2 (1 − 2χ v1 ) (1.58) 42 1 Introduction where v1 denotes the volume fraction of solvent in the solvent–polymer system and χ is the polymer–solvent interaction parameter, which is closely associated with the thermodynamics of polymer solution. The mutual diffusion coefficients with the polymer–solvent interaction parameter χ can be estimated by the groupcontribution lattice fluid model (Lee and Danner, 1996). The influence of moving phase boundary associated with the polymer swelling and diffusion-induced convection is considered to simulate the unsteady-state processes of water sorption by polymer (Alsoy and Duda, 2002). The effective diffusivity Deff is defined as ⎡ Deff = D0 ⎣(1 − ω1 ) ⎤2 0 V2 ⎦ (1.59) V where ω1 is the mass fraction of the solvent, V is the partial specific volume of 0 the mixture, V 2 is the initial partial specific volume of the polymer. In the above formulation, the effective diffusivity results from the moving boundary, the convective flows induced by diffusion, as well as the conventional, mutual binary diffusion coefficient. The studies show that, for most polymer–solvent systems, the influence of the diffusion-induced convection associated with the volume change in mixing may be neglected in analysis of sorption process. Free volume theories analyse the solute transport in terms of the free-volumebased topological analysis that incorporates the mesh size or correlation length of the three-dimensional structure. There is a significant dependence of the diffusion coefficients on the water concentration, which increases with increasing the water activity (Pradas et al., 2001). Diffusion of water in a polymer gel generally decreases with decreasing the degree of swelling. A small amount of water in the dry gel may be regarded as plasticizer and thus enhances the chain relaxation or relatively depresses the water penetration. By the pulsed field gradient NMR method, the water self-diffusion coefficient is measured for a set of nine commercially available contact lens hydrogels, where water content itself is the predominant factor in determining the water diffusion coefficient by an exponential decay using the specific binding model (McConville and Pope, 2000). No significant dependence of the mobility is found on polymer composition, which could not be related to equilibrium water content (McConville and Pope, 2001). The average mobility of the water in the hydrogels is largely dependent on the water content in the gel and increases with increasing the water content towards that of free water in phosphate buffered saline. From the long-time shrinking data of the DHPMA hydrogel, it is known that, as freezing water desorbs linearly with the square root of time, departure from linearity coincides with non-freezing water desorption (Gates et al., 2003). Additionally, Deff /D0 = (1 − xbw ) ξ is proposed (Manetti et al., 2002), in which the term ξ is the obstructive coefficient of the polymer material, xbw is the fraction of water molecules bound to the polymer network. 1.2 Historical Development of Modelling Hydrogel 43 Based on the Monte Carlo calculation, the following relation is obtained for the reduced diffusivities as a function of PVA volume fraction øPVA (Fergg and Keil, 2001): 0.154 − 0.18φPVA Deff = (1 − φPVA ) D0 0.1562 (1.60) By taking into account the variation of thickness due to swelling or shrinking and assuming a concentration-dependent diffusion coefficient, a model is developed as follows (Vicente and Gottifredi, 2000): M(τ ) = Cav (τ ) 1 + K(1 − CAV (τ )) (1.61) This model predicts the anomalous behaviour by taking into account the simultaneous polymer shrinking with Fickian diffusion. It is unnecessary to assume the presence of relaxation phenomena to explain the observed sigmoidal effect of volume change due to the uptake. 1.2.3 A Theoretical Formalism for Diffusion Coupled with Large Deformation of Hydrogel Apart from the above models discussed, a significant theoretical contribution to the modelling of polymer hydrogel has to be mentioned here. Recently Suo and his group developed a theoretical formalism for modelling of mass transport of small molecular species in three-dimensional polymeric network coupled with large deformation of the hydrogel (Hong et al., 2008), where there are two modes of large deformations. The first results from the fast process of local rearrangement of small molecules, allowing the change in shape but not volume of the hydrogel. The second results from slow process of long-range migration of the molecules, allowing the change in both shape and volume of the hydrogel. The present formalism is based on a nonequilibrium thermodynamic theory, where the network hydrogel swells as the small molecules mix with long polymeric chains so that the configurational entropy of the mixture increases while the configurational entropy of the network decreases. When the changes of the two entropies balance each other, the system of the hydrogel and solvent reaches equilibrium. In the theoretical formalism, a three-dimensional inhomogeneous field is characterized by the concentration of small molecular species C(X,t), deformation gradient FiK and free energy function W(F,C) as follows: FiK = ∂xi (X,t) ; W(F,C) = Ws (F) + Wm (C) ∂XK (1.62) 44 1 Introduction where X is the coordinate in reference state where the dry gel is not subjected to any mechanical load. In current state at time t, the marker X moves to a position with coordinate x(X, t). Ws (F) is the free energy due to network stretching and Wm (C) the free energy due to mixing of solvent and polymers. If a nominal stress sik (X,t) is defined as ∂ξi dV = Bi ξi dV + Ti ξi dA (1.63) siK ∂XK one can have the equilibrium condition of the system as δWdV = Bi δxi dV + Ti δxi dA + μδCdV (1.64) It leads to the equivalent equilibrium conditions as follows: siK = ∂W(F,C) ∂W(F,C) ∂siK ; ; μ= + Bi = 0; siK NK = Ti ∂FiK ∂C ∂XK (1.65) The theoretical formalism is based on the three assumptions as follows: (1) the volumetric change due to physical association is neglected; (2) the gel has no voids and (3) the individual solvent molecule and polymer are incompressible as 1 + υC = det (F) (1.66) where υ is the volume per solvent molecule and υC is the volume of the small molecules in the hydrogel divided by the volume of the dry polymers. The above molecular incompressibility condition (1.66) can be enforced as a constraint by introducing a Lagrange multiplier (X,t), namely W = W(F,C) + [1 + υC − det (F)] (1.67) Then one can have the equations of state as siK = ∂W(F,C) ∂W(F,C) + υ − HiK det (F); μ = ∂FiK ∂C (1.68) and the true stress as σij = ∂W(F,C) FjK − δij ∂FiK det (F) (1.69) where can be interpreted as the osmotic pressure that increases the chemical potential of the solvent entering the hydrogel. This theoretical formalism represents a significant progression. It opens a general form of formulas for the free energy function W(F,C) and kinetic law, both being material specific, such that it is applicable for modelling of solvent diffusion coupled with large deformation of various polymeric hydrogels. 1.3 About This Monograph 45 1.2.4 Remarks In terms of the steady-sate modelling for simulation of the equilibrium of smart hydrogels, three macroscopic models and a microscopic molecular simulation are overviewed for description of equilibrium behaviours of the volume transition of the hydrogel. The thermodynamic models establish the relationship between the hydrogel structure and the overall behaviours of the volume transition in terms of the free energy change, the chemical potential or the related osmotic pressure. They provide a simple and qualitative approach for prediction of equilibrium of the volume transition of various hydrogels. The transport models account for the osmotic pressure, the electrical potential, the hydrogel stress, and thus the hydrogel volume transition by the mobile ion diffusive flux. They characterize both kinetics and equilibrium of volume transition behaviours of the hydrogels by diffusion equations with incorporation of different osmotic pressure expressions. The multiphase mixture model predicts the kinetics and equilibrium of the volume transition of the hydrogels by considering the frictional forces among three phases. The molecular simulation gives further understanding of the mechanisms of the volume transition of the hydrogels by simulating various interactions involved in the volume transition process of the hydrogels. However, its intensive computational requirement restricts its application to the hydrogels with small structure. Furthermore, several key parameters for model development are summarized and reviewed. It is suggested that additional chemical and structural complexities must be considered to integrate these key parameters. The volume transition of the hydrogels can be predicted accurately with more detailed approaches. In terms of the transient modelling for simulation of the kinetics of smart hydrogels, three models are examined to investigate the kinetics of the volume variation of fast response hydrogels. The phenomenal model based on the second order of reaction kinetics provides a simple approach for experimental data correlation. The power law model suggests a method to investigate the kinetic mechanisms. The multi-component diffusion model successfully incorporates the mechanical deformation and ion transport in the hydrogels to explain the kinetics of the volume variation of the hydrogels. In brief, the present survey of the developed models for investigation of volume variation of the smart hydrogels gives an outline of historical development of modelling smart hydrogels and provides a useful guide for further development of better mathematical models for simulation of the novel smart hydrogels subject to various environmental biostimuli. 1.3 About This Monograph This monograph provides a comprehensive and systematic study of mathematical model development and numerical simulation of the smart polymer hydrogels in BioMEMS environment, and it is based on the author’s works conducted over 46 1 Introduction the past years. Several basic assumptions throughout this monograph are made as follows: • the hydrogel has no voids; • all the three phases (polymeric network matrix, interstitial fluid and ionic species) are incompressible, and thus it is understood that the swelling/deswelling of the hydrogels results mainly from the variation of volume fraction of the fluid phase by absorbing/exuding the fluid; • the hydrogel is immersed in an unstirred solution in vibration-free experimental device, the bulk flow of fluid or hydrodynamic velocity can thus be eliminated and subsequently the convective flux is neglected; and • the pore of the hydrogel is narrow enough so that the diffusion dominates the transmission of flux. The monograph is divided into seven chapters and each chapter is further divided into sections to better organize the materials. Chapter 1 briefly introduces the definition and applications of the smart polymer hydrogels and provides a historical background of model development of the polymer hydrogels. Chapter 2 presents the model development and systematic parametric studies for the smart hydrogels in response to the change in pH of surrounding solution. After stating the basic considerations and hypotheses, a novel mathematical model, termed the multi-effect-coupling pH stimulus (MECpH) model, is developed for simulation of the pH stimulus-responsive hydrogels. Numerical simulations are carried out for analysis of influences of various hydrogel material properties and environmental conditions on the responsive performance of the pH-sensitive hydrogels in equilibrium state. In Chap. 3, a novel multiphysics model is developed for modelling and simulation of the smart hydrogels responsive to externally applied electric field, which is called the multi-effect-coupling electric stimulus (MECe) model. After imposing the boundary and initial conditions and numerically discretizing the nonlinear coupled partial differential governing equations, the model is validated well by comparison with experimental data extracted from published literature. Both the steady-state and transient simulations are conducted for analysis of the equilibrium and kinetics of the electric stimulus-responsive hydrogels. Correspondingly, parametric studies are done for further discussion of the electric-sensitive hydrogels in equilibrium and kinetics, respectively. It is well known that many pH-sensitive hydrogels are often able to be responsive to externally applied electric voltage simultaneously. In Chap. 4, the multi-effectcoupling pH-electric stimuli (MECpHe) model is presented for simulation of the smart hydrogels responding to the pH-electric coupled stimuli, when the hydrogels are immersed in pH buffer solution subject to externally applied electric voltage. Several case studies are made for understanding the influences of important material properties and environmental conditions on the responsive behaviour of the smart hydrogels to the pH-electric coupled stimuli. References 47 Chapter 5 focuses on the model development and numerical simulation of the smart hydrogels responding to environmental temperature. A novel multiphysics model is developed mathematically, consisting of nonlinear partial differential equations coupled with a transcendental equation, termed the multi-effect-coupling thermal stimulus (MECtherm) model. This is a steady-state model and the formulation is based on the thermodynamics equilibrium theory. After the numerical discretization and examination of the model for the temperature-sensitive hydrogels, the detailed parametric studies are conducted for several important material properties and environmental conditions. In addition, a transient model is presented for kinetics of the thermal stimulus-responsive neutral hydrogels and corresponding simulations are done for prediction of kinetics of the smart hydrogels. Chapter 6 briefs the author’s latest works on the development of two novel models for simulation of the smart hydrogels responsive to the glucose concentration and ionic strength of surrounding solutions, respectively. In Chap. 7, a transient modelling is presented for simulation of the controlled drug release from a non-swellable micro-hydrogel particle as delivery carrier. The mathematical model directly couples the drug dissolution with drug diffusion as two driving source forces for controlled drug release. The drugs diffuse and dissolute through the continuous matrix of the micro-hydrogel particle. Computational result is compared numerically with published experiment data and very good agreement is achieved. It is followed by numerical simulations for wide-range parametric studies of various environmental conditions and the properties of the micro-hydrogel particle delivery systems. References E.C. Achilleos, K.N. Christodoulou, I.G. Kevrekidis. (2001). A transport model for swelling of polyelectrolyte gels in simple and complex geometries. Computational and Theoretical Polymer Science, 11, 63–80. E.C. Achilleos, R.K. Prud’homme, K.N. Christodoulou, K.R. Gee, I.G. Kevrekidis. (2000). Dynamic deformation visualization in swelling of polymer gels. Chemical Engineering Science, 55, 3335–3340. S. Alsoy, J.L. Duda. (2002). Influence of swelling and diffusion-induced convection on polymer sorption processes. AIChE Journal, 48, 1849–1855. C. Alvarez-Lorenzo, A. Concheiro. (2002). Reversible adsorption by a pH- and temperaturesensitive acrylic hydrogel. Journal of Controlled Release, 80, 247–257. M. Annaka, Y. Amo, S. Sasaki, Y. Tominaga, K. Motokawa, T. Nakahira. (2002). Salt effect on volume phase transition of a gel. Physical Review E, 65, 031805-(8). M. Annaka, M. Tokita, T. Tanaka, S. Tanaka, T. Nakahira. (2000). The gel that memorizes phases. The Journal of Physical Chemistry, 112, 471–477. G. Astarita. (1989). Heat and mass transfer in solid polymer system. In: Transport Phenomena in Polymeric Systems, R.A. Mashelkar, A.S. Mujumdar, R. Kamal (Eds.) New York: Wiley, pp. 339–351. A.M. Atta. (2002). Swelling behaviors of polyelectrolyte hydrogels containing sulfonate groups. Polymers for Advanced Technologies, 13, 567–576. E.M. Aydt, R. Hentschke. (2000). Swelling of a model network: A Gibbs-ensemble molecular dynamics study. Journal of Chemical Physics, 112, 5480–5487. 48 1 Introduction S.K. Bajpai. (2000). Swelling-deswelling behavior of poly(acrylamide-co-maleic acid) hydrogels. Journal of Applied Polymer Science, 80, 2782–2789. A.K. Bajpai, A. Giri. (2002). Swelling dynamics of a macromolecular hydrophilic network and evaluation of its potential for controlled release of agrochemicals. Reactive and Functional Polymers, 53, 125–141. A.K. Bajpai, M. Shrivastava. (2000). Dynamic swelling behavior of polyacrylamide based three component hydrogels. Journal of Macromolecular Science: Pure and Applied Chemistry, A37, 1069–1088. A.K. Bajpai, M. Shrivastava. (2001). Water sorption dynamics of hydrophobic, ionizable copolymer gels. Journal of Scientific and Industrial Research India, 60, 131–140. A.K. Bajpai, M. Shrivastava. (2002a). Enhanced water sorption of a semi-interpenetrating polymer network (IPN) of poly(2-hydroxyethyl methacrylate) (PHEMA) and poly(ethylene glycol) (PEG). Journal of Macromolecular Science: Pure and Applied Chemistry, A39, 1069–1088. A.K. Bajpai, M. Shrivastava. (2002b). Water sorption dynamics of a binary copolymeric hydrogel of a-hydroxyethyl methacrylate (HEMA). Journal of Biomaterials Science – Polymer Edition, 13, 237–256. A.K. Bajpai, M. Shrivastava. (2002c). Swelling kinetics of a hydrogel of poly(ethylene glycol) and poly(acrylamide-co-styrene). Journal of Applied Polymer Science, 85, 1419–1428. B. Barriere, L. Leibler. (2003). Kinetics of solvent absorption and permeation through a highly swellable elastomeric network. Journal of Polymer Science Part B: Polymer Physics, 41, 166–182. A.R. Berens, H.B. Hopfenberg. (1978). Diffusion and relaxation in glassy polymer powders: 2. separation of diffusion and relaxation parameters. Polymer, 19, 489–496. J.P. Boisvert, A. Malgat, I. Pochard, C. Daneault. (2002). Influence of the counter-ion on the effective charge of polyacrylic acid in dilute condition. Polymer, 43, 141–148. P. Bouillot, B.A. Vincent. (2000). Comparison of the swelling behaviour of copolymer and interpenetrating network microgel particles. Colloid and Polymer Science, 278, 74–79. F. Castelli, G. Pitarresi, G. Giammona. (2000). Influence of different parameters on drug release from hydrogel systems to a biomembrane model. Evaluation by differential scanning calorimetry technique. Biomaterials, 21, 821–833. T. Caykara, U. Bozkaya, O. Kantoglu. (2003). Network structure and swelling behavior of poly(acrylamide/crotonic acid) hydrogels in aqueous salt solution. Journal of Polymer Science Part B: Polymer Physics, 41, 1656–1664. T. Caykara, C. Ozyurek, O. Kantoglu, O. Guven. (2000). Equilibrium swelling behavior of pHand temperature-sensitive poly(N-vinyl 2-pyrrolidone-g-citric acid) polyelectrolyte hydrogels. Journal of Polymer Science Part B: Polymer Physics, 38, 2063–2071. A.N. Chatterjee, Q. Yu, J.S. Moore, N.R. Aluru. (2003). Mathematical modeling and simulation of dissolvable hydrogels. Journal of Aerospace Engineering, 16, 55–64. J. Chen, K. Park. (2000). Synthesis of fast-swelling, superporous sucrose hydrogels. Carbohydrate Polymers, 41, 259–268. Y. Chen, M. Yi. (2001). Swelling kinetics and stimuli-responsiveness of poly(DMAEMA) hydrogels prepared by UV-irradiation. Radiation Physics and Chemistry, 61, 65–68. H.C. Chiu, A.T. Wu, Y.F. Lin. (2001). Synthesis and characterization of acrylic acidcontaining dextran hydrogels. Polymer, 42, 1471–1479. H.C. Chiu, Y.F. Lin, Y.H. Hsu. (2002a). Effects of acrylic acid on preparation and swelling properties of pH-sensitive dextran hydrogels. Biomaterials, 23, 1103–1112. H.C. Chiu, Y.F. Lin, S.H. Hung. (2002b). Equilibrium swelling of copolymerized acrylic acid-methacrylated dextran networks: Effects of ph and neutral salt. Macromolecules, 35, 5235–5242. C.S. Cho, Y.I. Jeong, S.K. Kim, J.W. Nah, M. Kubota, T. Komoto. (2000). Thermoplastic hydrogel based on hexablock copolymer composed of poly(-benzyl -glutamate) and poly(ethylene oxide). Polymer, 41, 5185–5193. References 49 K.F. Chou, C.C. Han, S. Lee. (2000). Water transport in 2-hydroxyethyl methacrylate copolymer irradiated by γ rays in air and related phenomena. Journal of Polymer Science Part B: Polymer Physics, 38, 659–671. W.Y. Chuang, T.H. Young, D.M. Wang, R.L. Luo, Y.M. Sun. (2000). Swelling behavior of hydrophobic polymers in water ethanol mixtures. Polymer, 41, 8339–8347. R.O.R. Costa, R.F.S. Freitas. (2002). Phase behavior of poly(N-isopropylacrylamide) in binary aqueous solutions. Polymer, 43, 5879–5885. A.M.A. Da Costa, A.M. Amado. (2000). Molecular interactions in polyacrylamide/lithium perchlorate hydrogel composites. Polymer, 41, 5361–5365. D. Dibbern-brunelli, T.D.Z. Atvars. (2000). Thermal transitions of poly(vinyl alcohol) hydrogel sensed by a fluorescent probe. Journal of Applied Polymer Science, 76, 815–824. S. Ji, J. Ding. (2002). The wetting process of a dry polymeric hydrogel. Polymer Journal, 34, 267–270. D. Dhara, P.R. Chatterji. (2000). Phase transition in linear and cross-linked poly(Nisopropylacrylamide) in water: Effect of various types of additives. Journal of Macromolecular Science, Part C: Polymer Reviews, C40, 51–68. E. Diez-Pena, I. Quijada-Garrido, J.M. Barrales-Rienda. (2002). On the water swelling behaviour of poly(N-isopropylacrylamide) [P(N-iPAAm)] poly(methacrylic acid) [P(MAA)] their random copolymers and sequential interpenetrating polymer networks (IPNs). Polymer, 43, 4341–4348. S. Durmaz, O. Okay. (2000). Acrylamide/2-acrylamido-2-methylpropane sulfonic acid sodium salt-based hydrogels synthesis and characterization. Polymer, 41, 3693–3704. M. Ebara, T. Aoyagi, K. Sakai, T. Okano. (2001). The incorporation of carboxylate groups into temperature-responsive poly(N-isopropylacrylamide)-based hydrogels promotes rapid gel shrinking. Journal of Polymer Science Part A: Polymer Chemistry, 39, 335–343. G.M. Eichenbaum, P.K. Kiser, D. Shah, W.P. Meuer, D. Needham, S.A. Simon. (2000). Alkali earth metal binding properties of ionic microgels. Macromolecules, 33, 4087–4093. D.J. Enscore, H.B. Hopfenberg, V.T. Stannett. (1977). Effect of particle size on the mechanism controlling n-hexane sorption in glassy polystyrene microspheres. Polymer, 18, 793–800. B. Erman, P.J. Flory. (1986). Critical phenomena and transitions in swollen polymer networks and in linear macromolecules. Macromolecules, 19, 2342–2353. G. Evmenenko, T. Budtova. (2000). Structure changes in hydrogels immersed in a linear polymer solution studied by SANS. Polymer, 41, 4943–4947. J. Fei, Z. Zhang, L. Gu. (2002). Bending behavior of electroresponsive poly(vinyl alcohol) and poly(acrylic acid) semi-interpenetrating network hydrogel fibres under an electric stimulus. Polymer International, 51, 502–509. F. Fergg, F.J. Keil. (2001). Diffusion and reactions of multicomponent electrolytes in poly(vinyl alcohol) hydrogels –– modeling and experiment. Chemical Engineering Science, 56, 1305–1315. L. Ferreira, M.M. Vidal, M.H. Gil. (2000). Evaluation of poly(2-hydroxyethyl methacrylate) gels as drug delivery systems at different pH values. International Journal of Pharmaceutics, 194, 169–180. P.J. Flory. (1953). Principles of Polymer Chemistry, Ithaca, New York: Cornell University Press. A. Fomenko, Z. Sedlakova, J. Plestil, M. Ilavsky. (2002). Phase transition in swollen gels: Part 32. Temperature transition in charged poly(N-isopropylmethacrylamide) hydrogels in water and aqueous NaCl solutions. Physical Chemistry Chemical Physics, 4, 4360–4367. M.W.C.P. Franse, K. te Nijenhuis. (2000). Crosslinking index, molecular weight distribution and rubber equilibrium shear modulus during polyfunctional crosslinking of existing polymer. Part 5. Primary polymer with a discrete distribution of the molecular weight. Journal of Molecular Structure, 554, 1–10. H. Furukawa. (2000). Effect of varying preparing-concentration on the equilibrium swelling of polyacrylamide gels. Journal of Molecular Structure, 554, 11–19. L.H. Gan, G.R. Deen, X.J. Loh, X.Y. Gan. (2001). New stimuli-responsive copolymers of N-acryloyl-N’-alkyl piperazine and methyl methacrylate and their hydrogels. Polymer, 42, 65–69. 50 1 Introduction G. Gates, J.P. Harmon, J. Ors, P. Benz. (2003). 2, 3-dihydroxypropyl methacrylate and 2hydroxyethyl methacrylate hydrogels: Gel structure and transport properties. Polymer, 44, 215–222. A.J. Galli, W.H. Brumage. (1983). The freely jointed chain in expanded form. Journal of Chemical Physics, 79, 2411. R.A. Gemeinhart, J. Chen, H. Park, K. Park. (2000). pH-Sensitivity of fast responsive superporous hydrogels. Journal of Biomaterials Science, Polymer Edition, 11, 1371–1380. P.E. Grimshaw, J.H. Nussbaum, A.J. Grodzinsky. (1990). Kinetics of electricity and chemically induced swelling in polyelectrolyte gels. Journal of Chemical Physics, 93, 4462–4472. C.M. Hansen. (2000). Hansen Solubility Parameters: A User’s Handbook, Boca Raton: CRC Press. J.P. Harmon, S. Lee, J.C.M. Li. (1987). Methanol treatment in PMMA: the effect of mechanical deformation. Journal of Polymer Science Part A: Polymer Chemistry, 25, 3215–3229. M.M. Hassan, C.J. Durning. (1999). Effects of polymer molecular weight and temperature on case II transport. Journal of Polymer Science Part B: Polymer Physics, 37, 3159–3171. D.J.T. Hill, N.G. Moss, P.J. Pomery, A.K. Whittaker. (2000). Copolymer hydrogels of 2-hydroxyethyl methacrylate with n-butyl methacrylate and cyclohexyl methacrylate synthesis characterization and uptake of water. Polymer, 41, 1287–1296. A. Hiroki, Y. Maekawa, M. Yoshida, K. Kubota, R. Katakai. (2001). Volume phase transitions of poly(acryloyl-L-proline methyl ester) gels in response to water-alcohol composition. Polymer, 42, 1863–1867. Y.P. Hong, Y.C. Bae. (2002). Phase behaviors of partially ionized hydrogels in aqueous salt solutions: Applicability of the modified double-lattice model. Journal of Polymer Science Part B: Polymer Physics, 40, 2333–2338. W. Hong, X. Zhao, J. Zhou, Z. Suo. (2008). A theory of coupled diffusion and large deformation in polymeric gels, Journal of the Mechanics and Physics of Solids, 56, 1779–1793. Y. Huang, I. Szleifer, N.A. Peppas. (2002). A molecular theory of polymer gels. Macromolecules, 35, 1373–1380. A. Huther, B. Schafer, X. Xu, G. Maurer. (2002). Phase equilibria of hydrogel systems. Physical Chemistry Chemical Physics, 4, 835–844. A. Ikehat, H. Ushiki. (2002). Effect of salt on the elastic modulus of poly(N-isopropylacrylamide) gels. Polymer, 43, 2089–2094. M. Ilavsky, G. Mamytbekov, L. Hanykova, K. Dusek. (2002). Phase transition in swollen gels: 31. Swelling and mechanical behaviour of interpenetrating networks composed of poly(1-vinyl2-pyrrolidone) and polyacrylamide in water/acetone mixtures. European Polymer Journal, 38, 875–883. K. Ito, Y. Ujihira, T. Yamashita, K. Horie. (2000). Temperature dependence of free volume of polyacrylamide gels studied by positron lifetime measurements. Radiation Physics and Chemistry, 58, 521–524. E. Jabbari, S. Nozari. (2000). Swelling behavior of acrylic acid hydrogels prepared by γradiation crosslinking of polyacrylic acid in aqueous solution. European Polymer Journal, 36, 2685–2692. B.D. Johnson, D.J. Niedermaier, W.C. Crone, J. Moorthy, D.J. Beebe. (2002). Mechanical properties of a pH sensitive hydrogel, Proceedings of the 2002 Annual Conference of Society for Experimental Mechanics, Milwaukee, Wisconsin. E. Karadag, D. Saraydin. (2002). Swelling of superabsorbent acrylamide/sodium acrylate hydrogels prepared using multifunctional crosslinkers. Turkish Journal of Chemistry, 26, 863–875. I. Katime, E.D. de Apodaca. (2000). Acrylic acid/methyl methacrylate hydrogels. I. Effect of composition on mechanical and thermodynamic properties. Journal of Macromolecular Science: Pure and Applied Chemistry, A37, 307–321. I. Katime, E. Rodriguez. (2001). Absorption of metal ions and swelling properties of poly(acrylic acid-co-itaconic acid) hydrogels. Journal of Macromolecular Science: Pure and Applied Chemistry, A38, 543–558. N.R. Kenkare, C.K. Hall, S.A. Khan. (2000). Theory and simulation of the swelling of polymer gels. Journal of Physical Chemistry, 113, 404–418. References 51 M.N. Khalid, F. Agnely, N. Yagoubi, J.L. Grossiord, G. Couarraze. (2002). Water state characterization, swelling behavior, thermal and mechanical properties of chitosan based networks. European Journal of Pharmaceutical Sciences, 15, 425–432. A.R. Khokhlov, E. Yu. Kramarenko. (1994). Polyelectrolyte/Ionomer behavior in polymer gel collapse. Macromolecular Theory and Simulations, 3, 45–59. S.J. Kim, S.J. Park, I.Y. Kim, M.S. Shin, S.I. Kim. (2002). Electric stimuli responses to poly(vinyl alcohol)/chitosan interpenetrating polymer network hydrogel in NaCl solutions. Journal of Applied Polymer Science, 86, 2285–2289. S.J. Kim, S.J. Park, S.I. Kim. (2003a). Synthesis and characteristics of interpenetrating polymer network hydrogels composed of poly(vinyl alcohol) and poly(N-isopropylacrylamide). Reactive and Functional Polymers, 55, 61–67. B. Kim, N.A. Peppas. (2002). Complexation phenomena in pH-responsive copolymer networks with pendent saccharides. Macromolecules, 35, 9545–9550. S.J. Kim, G.Y. Yoon, Y.M. Lee, S.I. Kim. (2003b). Electrical sensitive behavior of poly(vinyl alcohol)/poly(diallyldimethylammonium chloride) IPN hydrogel. Sensors and Actuators B: Chemical, 88, 286–291. J. Kovac. (1978). Modified Gaussian model for rubber elasticity. Macromolecules, 11, 362–365. E. Yu. Kramarenko, A.R. Khokhlov, K. Yoshikawa. (2000). A three-state model for counterions in a dilute solution of weakly charged polyelectrolytes. Macromolecular Theory and Simulations, 9, 249–256. K.Y. Lee, K.H. Bouhadir, D.J. Mooney. (2000). Degradation behavior of covalently cross-linked poly(aldehyde guluronate) hydrogels. Macromolecules, 33, 97–101. W.F. Lee, Y.J. Chen. (2001). Studies on preparation and swelling properties of the Nisopropylacrylamide/chitosan semi-IPN and IPN hydrogels. Journal of Applied Polymer Science, 82, 2487–2496. B.C. Lee, R.P. Danner. (1996). Application of the group-contribution lattice-fluid equation of state to random copolymer-solvent systems, Fluid Phase Equilibria, 117, 33–39. W.F. Lee, Y.H. Lin. (2001). pH-reversible hydrogels. IV. Swelling behavior of the 2-hydroxyethyl methacrylate-co-acrylic acid-co-sodium acrylate copolymeric hydrogels. Journal of Applied Polymer Science, 81, 1360–1371. J. Lee, C.W. Marcosko, D.W. Urry. (2001). Phase transition and elasticity of protein-based hydrogels. Journal of Biomaterials Science – Polymer Edition, 12, 229–242. W.F. Lee, P.L. Yeh. (2000). Thermoreversible hydrogels. IX. Swelling behaviors of thermosensitive hydrogels copolymerized by N-isopropylacrylamide with 1-vinyl-3-(3-sulfopropyl) imidazolium betaine. Journal of Applied Polymer Science, 77, 14–23. B. Li, D. Ding, P. Sun, Y. Wang, J. Ma, B. He. (2000). PGSE NMR studies of water states of hydrogel P(Am-NaA). Journal of Applied Polymer Science, 77, 424–427. T. Lindvig, M.L. Michelsen, G.M. Kontogeorgis. (2002). A Flory–Huggins model based on the Hansen solubility parameters. Fluid Phase Equilibria, 5093, 1–14. V.M.M. Lobo, A.J.M. Valente, A.Y. Polishchuk, G. Geuskens. (2001). Transport of non-associated electrolytes in acrylamide hydrogels. Journal of Molecular Liquids, 94, 179–192. X.J. Loh, G.R. Deen, X.Y. Gan, L.H. Gan. (2001). Water-sorption and metal-uptake behavior of pH-responsive poly(N-acryloyl-N’-methylpiperazine) gels. Journal of Applied Polymer Science, 80, 268–273. Z.Y. Lu, R. Hentschke. (2002a). Computer simulation study on the swelling of a model polymer network by a chainlike solvent. Physical Review E, 65, 041807. Z.Y. Lu, R. Hentschke. (2002b). Swelling of model polymer networks with different cross-link densities: A computer simulation study. Physical Review E, 66, 041803. X. Lu, M. Zhai, J. Li, H. Ha. (2000). Radiation preparation and thermo-response swelling of interpenetrating polymer network hydrogel composed of PNIPAAm and PMMA. Radiation Physics and Chemistry, 57, 477–480. A.V. Lyulin, B. Dunweg, O.V. Borisov, A.A. Darinskii. (1999). Computer simulation studies of a single polyelectrolyte chain in poor solvent. Macromolecules, 32, 3264–3278. 52 1 Introduction T.M. Madkour. (2001). A combined statistical mechanics and molecular dynamics approach for the evaluation of the miscibility of polymers in good, poor and non-solvents. Chemical Physics, 274, 187–198. K. Makino, H. Agata, H. Ohshima. (2000a). Dependence of temperature-sensitivity of poly(Nisopropylacrylamide-co-acrylic acid) hydrogel microspheres upon their sizes. Journal of Colloid and Interface Science, 230, 128–134. K. Makino, J. Hiyoshi, H. Ohshima. (2000b). Kinetics of swelling and shrinking of poly(N-isopropylacrylamide) hydrogels at different temperatures. Colloids and Surfaces B: Biointerfaces, 19, 197–204. C. Manetti, L. Casciani, N. Pescosolido. (2002). Diffusive contribution to permeation of hydrogel contact lenses theoretical model and experimental evaluation by nuclear magnetic resonance techniques. Polymer, 43, 87–92. F. Martellini, L.H.I. Mei, J.L. Balino, M. Carenza. (2002). Swelling and water transport in temperature-sensitive hydrogels based on 2-methoxyethylacrylate. Radiation Physics and Chemistry, 63, 29–33. P. Martens, K.S. Anseth. (2000). Characterization of hydrogels formed from acrylate modified poly(vinyl alcohol) macromers. Polymer, 41, 7715–7722. A. Matsuda, Y. Katayama, T. Kaneko, J.P. Gong, Y. Osada. (2000). Ionization and order–disorder transition of hydrogels with ionizable hydrophobic side chain. Journal of Molecular Structure, 554, 91–97. P. McConville, J.M. Pope. (2000). A comparison of water binding and mobility in contact lens hydrogels from NMR measurements of the water self-diffusion coefficient. Polymer, 41, 9081–9088. P. McConville, J.M. Pope. (2001). 1 H NMR T2 relaxation in contact lens hydrogels as a probe of water mobility. Polymer, 42, 3559–3568. J.R. Meakin, D.W.L. Kukins, C.T. Imrie, R.M. Aspden. (2003). Thermal analysis of poly(2hydroxyethyl methacrylate) (pHEMA) hydrogels. Journal of Materials Science: Materials in Medicine, 14, 9–15. D. Melekaslan, O. Okay. (2000). Swelling of strong polyelectrolyte hydrogels in polymer solutions: Effect of ion pair formation on the polymer collapse. Polymer, 41, 5737–5747. D. Melekaslan, O. Okay. (2001). Reentrant phase transition of strong polyelectrolyte poly(Nisopropylacrylamide) gels in PEG solutions. Macromolecular Chemistry and Physics, 202, 304–312. V. Michailova, S. Titeva, R. Kotsilkova, E. Krusteva, E. Minkov. (2000). Water uptake and relaxation processes in mixed unlimited swelling hydrogels. International Journal of Pharmaceutics, 209, 45–56. E.C. Muniz, G. Geuskens. (2001). Influence of temperature on the permeability of polyacrylamide hydrogels and semi-IPNs with poly(N-isopropylacrylamide). Journal of Membrane Science, 172, 287–293. H. Muta, K. Ishida, E. Tamaki, M. Satoh. (2002). An IR study on ion-specific and solvent-specific swelling of poly(N-vinyl-2-pyrrolidone) gel. Polymer, 43, 103–110. H. Muta, R. Kojima, S. Kawauchi, A. Tachibana, M. Satoh. (2001a). Ion-specificity for hydrogenbonding hydration of polymer: An approach by ab initio molecular orbital calculations. Journal of Molecular Structure: THEOCHEM, 536, 219–226. H. Muta, M. Miwa, M. Satoh. (2001b). Ion-specific swelling of hydrophilic polymer gels. Polymer, 42, 6313–6138. H. Muta, T. Sin, A. Yamanaka, S. Kawauchi, M. Satoh. (2001c). Ion-specificity for hydrogenbonding hydration of polymer: An approach by ab initio molecular orbital calculations II. Journal of Molecular Structure: THEOCHEM, 574, 195–211. B. Nick, U.W. Suter. (2001). Solubility of water in polymers-atomistic simulations. Computational and Theoretical Polymer Science, 11, 49–54. T. Norisuye, N. Masui, Y. Kida, D. Ikuta, E. Kokufuta, S. Ito, S. Panyukov, M. Shibayama. (2002). Small angle neutron scattering studies on structural inhomogeneities in polymer gels: irradiation cross-linked gels vs chemically crosslinked gels. Polymer, 43, 5289–5297. References 53 K. Ogawa, Y. Ogawa, E. Kokufuta. (2002). Effect of charge inhomogeneity of polyelectrolyte gels on their swelling behavior. Colloids and Surfaces A: Physicochemical and Engineering Aspects, 209, 267–279. R.R. Ohs, S.K. De, N.R. Aluru. (2001). Modelling of ionic hydrogel kinetics in buffered solutions, Technical Proceedings of the 2001 International Conference on Modeling and Simulation of Microsystems, 1, 7–10. O. Okay, S. Durmaz. (2002). Charge density dependence of elastic modulus of strong polyelectrolyte hydrogels. Polymer, 43, 1215–1221. O. Okay, S.B. Sariisik. (2000). Swelling behavior of poly(acrylamide-co-sodium acrylate) hydrogels in aqueous salt solutions: Theory versus experiments. European Polymer Journal, 36, 393–399. D. Ostrovskii, M. Edvardsson, P. Jacobsson. (2003). Weak polymer-electrolyte interaction revealed by Fermi resonance perturbed Raman bands. Journal of Raman Spectroscopy, 34, 40–49. M.M. Ozmen, O. Okay. (2003). Swelling behavior of strong polyelectrolyte poly(N-tbutylacrylamide-co-acrylamide) hydrogels. European Polymer Journal, 39, 877–886. V. Ozturk, O. Okay. (2002). Temperature sensitive poly(N-t-butylacrylamide-co-acrylamide) hydrogels synthesis and swelling behavior. Polymer, 43, 5017–5026. A. Panda, S.B. Manohar, S. Sabharwal, Y.K. Bhardwaj, A.B. Majali. (2000). Synthesis and swelling characteristics of poly (N-isopropylacrylamide) temperature sensitive hydrogels crosslinked by electron beam irradiation. Radiation Physics and Chemistry, 58, 101–110. S. Panyukov, Y. Rabin. (1996). Statistical physics of polymer gels. Physics Reports, 269, 1–131. N.A. Peppas. (1986). Hydrogels in Medicine and Pharmacy, Boca Raton, FL: CRC Press. K. Podual, N.A. Peppas. (2005). Relaxational behavior and swelling-pH master curves of poly[(diethylaminoethyl methacrylate)-graft-(ethylene glycol)] hydrogels. Polymer International, 54, 581–593. M.M. Pradas, J.L.G. Ribelles, A.S. Aroca, G.G. Ferrer, J.S. Anton, P. Pissis. (2001). Porous poly(2hydroxyethyl acrylate) hydrogels. Polymer, 42, 4667–4674. X. Qu, A. Wirsen, A.C. Albertsson. (2000). Novel pH-sensitive chitosan hydrogels swelling behavior and states of water. Polymer, 41, 4589–4598. J.R. Quintana, N.E. Valderruten, N.E. Katime. (1999). Synthesis and swelling kinetics of poly(dimethylaminoethyl acrylate methyl chloride quaternary-co-itaconic acid) hydrogels. Langmuir, 15, 4728–4730. G.V.N. Rathna, P.R. Chatterji. (2001). Swelling kinetics and mechanistic aspects of thermosensitive interpenetrating polymer networks. Journal of Macromolecular Science: Pure and Applied Chemistry, A38, 43–56. T. Schmidt, C. Querner, K.F. Arndt. (2003). Characterization methods for radiation crosslinked poly(vinyl methyl ether) hydrogels. Nuclear Instruments and Methods in Physics Research Section B: Beam Interactions with Materials and Atoms, 208, 331–335. H. Schott. (1992). Swelling kinetics of polymers. Journal of Macromolecular Science: Physics, B31, 1–9. U.P. Schroder, W. Oppermann. (2002). Computer simulation of network formation via crosslinking copolymerization. Macromolecular Theory and Simulations, 6, 151–160. M. Sen, O. Güven. (1998). Prediction of swelling behaviour of hydrogels containing diprotic acid moieties. Polymer, 39, 1165–1172. M. Sen, O. Güven. (2000). Prediction of the swelling behavior of amphiphilic hydrogels and the determination of average molecular weight between cross-links. Computational and Theoretical Polymer Science, 11, 475–482. M. Sen, O. Guven. (2002). Dynamic deswelling studies of poly(N-vinyl-2-pyrrolidone/itaconic acid) hydrogels swollen in water and terbinafine hydrochloride solutions. European Polymer Journal, 38, 751–757. B.C. Shin, S.S. Kim, J.K. Ko, J. Jegal, B.M. Lee. (2003). Gradual phase transition of poly(Nisopropylacrylamide-co-acrylic acid) gel induced by electric current. European Polymer Journal, 39, 579–584. 54 1 Introduction M.R. Simmons, E.N. Yamasaki, C.S. Patrickios. (2000). Cationic amphiphilic model networks: Synthesis by group transfer polymerization and characterization of the degree of swelling. Macromolecules, 33, 3176–3179. Y. Suetoh, M. Shibayama. (2000). Effects of non-uniform solvation on thermal response in poly(Nisopropylacrylamide) gels. Polymer, 41, 505–510. T. Tokuhiro. (2001). Temperature dependence of density of polymer gels: 2. Poly[N-(1,3-dioxolan2-ylmethyl)-N-methyl-acrylamide] networks -water or -alcohol system. Journal of Physical Chemistry B, 105, 11955–11960. A.I. Triftaridou, S.C. Hadjiyannakou, M. Vamvakaki, C.S. Patrickios. (2002). Synthesis, characterization, and modelling of cationic amphiphilic model hydrogels: Effects of polymer composition and architecture. Macromolecules, 35, 2506–2513. J. Valencia, I.F. Pierola. (2001). Equilibrium swelling properties of poly(N-vinylimidazole-cosodium styrenesulfonate) hydrogels. European Polymer Journal, 37, 2345–2352. J. Valencia, I.F. Pierola. (2002). Swelling kinetics of poly(N-vinylimidazole-co-sodium styrenesulfonate) hydrogels. Journal of Applied Polymer Science, 83, 191–200. A.J.M. Valente, A.Y. Polishchuk, V.M.M. Lobo, G. Geuskens. (2002). Diffusion coefficients of lithium chloride and potassium chloride in hydrogel membranes derived from acrylamide. European Polymer Journal, 38, 13–18. S. Varghese, A.K. Lele, R.A. Masjelkar. (2000). Designing new thermoreversible gels by molecular tailoring of hydrophilic-hydrophobic interactions. Journal of Physical Chemistry, 112, 3063–3070. E.V. Vashuk, E.V. Vorobieva, I.I. Basalyga, N.P. Krutko. (2001). Water-absorbing properties of hydrogels based on polymeric complexes. Materials Research Innovations, 4, 350–352. M.S. Vicente, J.C.Y. Gottifredi. (2000). Effect of volume changes due to absorption in polymer membranes. Journal of Membrane Science, 169, 249–254. J.S. Vrentas, C.M. Vrentas. (1994). Solvent self-diffusion in rubbery polymer-solvent systems. Macromolecules, 27, 4684–4690. T. Wallmersperger, B. Kroplin, J. Holdenried, W. Gulch. (2001). A Coupled Multi-FieldFormulation for Ionic Polymer Gels in Electric Fields. In: Smart Structures and Materials 2001: Electroactive Polymer Actuators and Devices, Y. Bar-Cohen (Ed.) SPIE Press, 4329, pp. 264–275. B. Wang, T. Ymaguchi, S. Nakao. (2000). Solvent diffusion in amorphous glassy polymers. Journal of Polymer Science Part B: Polymer Physics, 38, 846–856. J.A. White, W.M. Deen. (2002). Agarose-dextran gels as synthetic analogs of glomerular basement membrane water permeability. Biophysical Journal, 82, 2081–2089. C.J. Whiting, A.M. Voice, P.D. Olmsted, T.C.B. Mcleish. (2001). Shear modulus of polyelectrolyte gels under electric field. Journal of Physics: Condensed Matter, 13, 1381–1393. W. Xue, S. Champ, M.B. Huglin. (2001a). Thermoreversible swelling behaviour of hydrogels based on N-isopropylacrylamide with a zwitterionic comonomer. European Polymer Journal, 37, 869–875. W. Xue, S. Champ, M.B. Huglin. (2001b). Network and swelling parameters of chemically crosslinked thermoreversible hydrogels. Polymer, 42, 3665–3669. W. Xue, I.W. Hamley. (2002). Thermoreversible swelling behaviour of hydrogels based on Nisopropylacrylamide with a hydrophobic comonomer. Polymer, 43, 3069–3077. L. Yao, S. Krause. (2003). Electromechanical responses of strong acid polymer gels in DC electric fields. Macromolecules, 36, 2055–2065. H. Yasunaga, Y. Shirakawa, H. Urakawa, K. Kajiwara. (2002). Dynamic behaviour of water in hydrogel containing hydrophobic side chains as studied by pulse 1 H NMR. Journal of Molecular Structure, 602–603, 399–404. B. Yildiz, B. Isik, M. Kis. (2002). Thermoresponsive poly(N-isopropylacrylamide-co-acrylamideco-2-hydroxyethyl methacrylate) hydrogels. Reactive and Functional Polymers, 52, 3–10. M.K. Yoo, Y.K. Sung, Y.M. Lee, C.S. Cho. (2000). Effect of polyelectrolyte on the lower critical solution temperature of poly(N-isopropyl acrylamide) in the poly(NIPAAm-co-acrylic acid) hydrogel. Polymer, 41, 5713–5719. References 55 L. Zha, J. Hu, C. Wang, S. Fu, M. Luo. (2002). The effect of electrolyte on the colloidal properties of poly(N-isopropylacrylamide-co-dimethylaminoethylmethacrylate) microgel latexes. Colloid and Polymer Science, 280, 1116–1121. J. Zhang, N.A. Peppas. (2000). Synthesis and characterization of pH- and temperature-sensitive poly(methacrylic acid)/poly(N-isopropylacrylamide) interpenetrating polymeric networks. Macromolecules, 33, 102–107. X.Z. Zhang, D.Q. Wu, C.C. Chu. (2003). Effect of the crosslinking level on the properties of temperature-sensitive poly(N-isopropylacrylamide) hydrogels. Journal of Polymer Science Part B: Polymer Physics, 41, 582–593. X.Z. Zhang, R.X. Zhuo. (2000a). Preparation of fast responsive, thermally sensitive poly(Nisopropylacrylamide) gel. European Polymer Journal, 36, 2301–2303. X.Z. Zhang, R.X. Zhuo. (2000b). Novel synthesis of temperature-sensitive poly(Nisopropylacrylamide) hydrogel with fast deswelling rate. European Polymer Journal, 36, 643–645. X.Z. Zhang, R.X. Zhuo. (2000c). Synthesis of temperature-sensitive poly(N-isopropylacrylamide) hydrogel with improved Surface Property. Journal of Colloid and Interface Science, 223, 311–313. X.Z. Zhang, R.X. Zhuo. (2002). Synthesis, properties of thermosensitive poly(Nisopropylacrylamide-co-methyl methacrylate) hydrogel with rapid response. Materials Letters, 52, 5–9. B. Zhao, J.S. Moore. (2001). Fast pH- and ionic strength-responsive hydrogels in microchannels. Langmuir, 17, 4758–4763. X. Zhou, Y.C. Hon, S. Sun, A.F.T. Mak. (2002). Numerical simulation of the steady-state deformation of a smart hydrogel under an external electric field. Smart Materials and Structures, 11, 459–467.